# institut fu¨r physik, johannes gutenberg-universit¨at, d

Embed Size (px)

TRANSCRIPT

compared to theoretical predictions

Hsiao-Ping Hsu, Wolfgang Paul, and Kurt Binder Institut fur Physik, Johannes Gutenberg-Universitat, D-55099 Mainz, Germany

Summary: Scaling predictions and results from self- consistent field calculations for bottle-brush polymers with a rigid backbone and flexible side chains under good solvent conditions are summarized and their validity and applicability is assessed by a comparison with Monte Carlo simulations of a simple lattice model. It is shown that under typical conditions, as they are also present in experiments, only a rather weak stretching of the side chains is realized, and then the scaling predictions based on the extension of the Daoud-Cotton blob picture are not applicable.

Also two-component bottle brush polymers are consid- ered, where two types (A,B) of side chains are grafted, as- suming that monomers of different kind repel each other. In this case, variable solvent quality is allowed for, such that for poor solvent conditions rather dense cylinder- like structures result. Theories predict “Janus Cylinder”- type phase separation along the backbone in this case. The Monte Carlo simulations, using the pruned-enriched Rosenbluth method (PERM) then are restricted to rather short side chain length. Nevertheless, evidence is ob- tained that the phase separation between an A-rich part of the cylindrical molecule and a B-rich part can only occur locally. The correlation length of this microphase separation can be controlled by the solvent quality. This lack of a phase transition is interpreted by an analogy with models for ferromagnets in one space dimension.

I. Introduction

Flexible macromolecules can be grafted to various sub- strates by special endgroups. Such “polymer brushes” find widespread applications[1, 2, 3, 4, 5] and also pose challenging theoretical problems, such as an understand- ing of the conformational statistics and resulting geomet- rical structure of these tethered chain molecules. Only this latter aspect shall be considered in the present pa- per, for chains grafted to a straight line or a very nar- row cylinder. This problem is a limiting case of “bot- tle brush” polymers where side chains are grafted to a long macromolecule that forms the backbone of the bot- tle brush. When this backbone chain is also a flexible polymer and the grafting density is not very high, a “comb polymer”[6] results, which is outside of consider- ation here. Also we shall not discuss the case where the backbone chain is very short, so the conformation would resemble a “star polymer”.[7, 8, 9, 10, 11] Here we restrict attention to either stiff backbone chains or high graft- ing density of side chains at flexible backbones. In the

lattice case stiffening of the backbone occurs due to ex- cluded volume interactions, and a cylindrical shape of the molecule as a whole results. In fact, many experiments have been carried out where with an appropriate chemical synthesis bottle brush polymers with a worm-like cylin- drical shape were produced [12, 13, 14, 15, 16]. The recent papers[14, 15, 16] contain a more detailed bibliography on this rapidly expanding field. On the theoretical side, two aspects of the confor-

mation of bottle brush polymers where mostly dis- cussed: (i) conformation of a side chain when the back- bone can be treated as a rigid straight line or thin cylinder[10, 17, 18, 19, 20, 21, 22, 23, 24, 25, 26, 27] (ii) confor- mation of the whole bottle brush when the backbone is (semi)flexible.[28, 29, 30, 31, 32, 33, 34, 35, 36, 37, 38, 39, 40]

The latter problem is left out of consideration in the present paper. Problem (i), the stretching of the side chains in the radial direction in the case of sufficiently high grafting density, was mostly discussed in terms of a scaling description, [10, 17, 18, 19, 20, 24, 25, 26] extending the Daoud-Cotton [8] “blob picture”[41, 42, 43] from star polymers to bottle brush polymers. If one uses the Flory exponent[44, 45] ν = 3/5 in the scaling relation for the average root mean square end-to-end distance of a side chain, Re ∝ σ(1−ν)/(1+ν)N2ν/(1+ν), where σ is the graft- ing density and N is the number of effective monomeric units of a side chain, one obtains Re ∝ σ1/4N3/4. These exponents happen to be identical to those which one would obtain assuming that the chains attain quasi- two-dimensional configurations, resulting if each chain is confined to a disk of width σ−1.[27] Although this lat- ter picture is a misconception, in experimental studies (e.g. [14, 15]) this hypothesis of quasi-two-dimensional chains is discussed as a serious possibility. Therefore we find it clearly necessary to first review the correct scaling theory based on the blob picture, and discuss in detail what quantities need to be recorded in order to distin- guish between these concepts. Thus, in the next section we shall give a detailed discussion of the scaling concepts for bottle brush polymers with rigid backbones. Thereafter we shall describe the Monte Carlo test

of these predictions, that we have recently per- formed using the pruned enriched Rosenbluth method (PERM).[46, 47, 48, 49] After a brief description of the Monte Carlo methodology, we present our numerical re- sults and compare them to the pertinent theoretical pre- dictions. In the second part of this paper, we discuss the

extension from one-component to two-component bot- tle brush polymers. Just as in a binary polymer blend (A,B) typically the energetically unfavorable in-

teraction (described by the Flory-Huggins parameter χ [44, 45, 50, 51, 52]) should cause phase separation be- tween A-rich and B-rich domains. However, just as in block copolymers where A chains and B-chains are tethered together in a point,[53, 54, 55] no macroscopic phase separation but only “microphase separation” is possible: for a binary (A,B) bottle brush with a rigid backbone one may expect formation of “Janus Cylin- der” structures.[56, 57, 58] This means, phase separation occurs such that the A-chains assemble in one half of the cylinder, the B chains in the other half, separated from the A-chains via a flat interface containing the cylinder axis. However, it has been argued that the long range order implied by such a “Janus cylinder” type struc- ture has a one-dimensional character, and therefore true long range order is destroyed by fluctuations at nonzero temperature.[58] Only local phase separation over a finite correlation length along the cylinder axis may persist.[58]

We shall again first review the theoretical background on this problem, and then describe the simulation evi- dence. We conclude our paper by a summary and out- look on questions that are still open, briefly discussing also possible consequences on experimental work. How- ever, we shall not deal with the related problems of mi- crophase separation of a bottle brush with only one kind of side chains induced by deterioration of the solvent quality[59, 60] or by adsorption on flat substrates.[61, 62, 63]

II. Conformation of Side Chains of Bottle Brushes under Good Solvent Conditions: Theoretical Background

The most straightforward approach to understand the conformations of chains in polymer brushes and star polymers under good solvent conditions uses the con- cept to partition the space available for the chains into compartments, called “blobs”. The idea is that in each such region there occur only monomers of one chain, no monomers of any other chains occur in such a blob, and hence self-avoiding walk statistics holds in each blob. This means, if a (spherical) blob has a radius rB and contains n monomers, these numbers must be related via

rB = anν , ν ≈ 0.588 , n 1 . (1)

Here a is a length of the order of the size of an effec- tive monomer, and we emphasize from the start that it is crucial to use the correct value of the self-avoiding walk exponent ν, as it is provided from renormalization group calculations[64] or accurate Monte Carlo simulations.[65]

If one would ignore the small difference between ν and the Flory estimate 3/5, one would already miss an impor- tant distinction between two different scaling regimes for a brush on a flat substrate.[66] An almost trivial condi- tion of this “blobology”[43] is that each of the N effective monomeric units of a chain must belong to some blob.

So we have

N = nnB , (2)

where nB is the number of blobs belonging to one par- ticular chain. Finally we note that the space available to the chains

must be densely filled with blobs. It then remains to discuss which factors control the blob size rB.

[43] The simplest case is a polymer brush on a flat substrate (un- der good solvent conditions, as assumed here through- out): if we neglect, for simplicity, any local fluctuations in the grafting density, the distance between grafting sites simply is given by σ−1/2. Putting rB = σ−1/2 in Equation (1), we find n = (σa2)−1/2ν , i.e. each chain is a string of nB = N/n = N(σa2)1/2ν blobs. Accord- ing to the simple-minded description of polymer brushes due to Alexander,[41] this string simply is arranged like a one-dimensional cigar, and one would conclude that the height of a flat brush is

h = σ−1/2nB = Na(σa2)1/(2ν)−1/2 . (3)

The free end of the chain is in the last blob and hence the end-to-end distance Re ≈ h in this “Alexander picture” of polymer brushes.[1, 41, 42, 43] However, a more detailed theory of polymer brushes, such as the self-consistent field theory in the strong stretching limit,[67, 68, 69] yields a somewhat different behavior: the end monomer is not localized at the outer edge of the brush, but rather can be located anywhere in the brush, according to a broad dis- tribution; also the monomer density in polymer brushes at flat substrates is not constant up to the brush height h, but rather decreases according to a parabolic profile. So even for a polymer brush at a flat substrate already a description in terms of non-uniform blob sizes, that increase with increasing distance z from the substrate, is required.[70] However, in the following we shall disre- gard all these caveats about the Alexander picture for flat brushes, and consider its generalization to the bottle brush geometry, where polymer chains are tethered to a line rather than a flat surface. Then we have to partition space into blobs of nonuniform size and shape in order to respect the cylindrical geometry (Figure 1). In the discussion of brushes in cylindrical geometry in

terms of blobs in the literature[19, 20, 26] the non-spherical character of the blob shape is not explicitly accounted for, and it rather is argued that one can characterize the blobs by one effective radius ξ(r) depending on the radial dis- tance r from the cylinder axis. One considers a segment of the array of length L containing p polymer chains.[19]

On a surface of a cylinder of radius r and length L there should then be p blobs, each of cross-sectional area ξ2(r); geometrical factors of order unity are ignored throughout. Since the surface area of the cylindrical segment is Lr, we must have[19, 20, 26]

pξ2(r) = Lr , ξ(r) = (Lr/p)1/2 = (r/σ)1/2 . (4)

If the actual non-spherical shape of the blobs (Figure 1) is neglected, the blob volume clearly is of the order of

3

r

(b)

FIG. 1: Schematic construction of a blob picture for star polymer (a), and for a bottle brush (b), (c). We assume that along the rigid backbone there occur at a regular spacing fσ−1 grafting sites where at each grafting site f side chains containing N effective monomeric units are grafted. If the rigid backbone of the cylindrical bottle brush is oriented along the z-axis, part (c) shows a view of the blob partitioning in the xy-plane perpendicular to the backbone, while part (b) shows a cut through the cylinder along the xz-plane containing the cylinder axis. A few possible chain configurations are indicated. While for a star polymer the blobs have a spherical shape, their radius ξ(r) increasing linearly proportional to the distance r from the center of the star (a), for the bottle brush the blobs are ellipsoids with three axes ξ(r) (in x-direction), proportional to r/f (in y-direction), and fσ−1 (in z-direction), respectively. For a considered chain the x-axis contains the center of mass of the chain.

ξ3(r) = (r/σ)3/2. Invoking again the principle that in- side a blob self-avoiding walk statistics hold, we have, in analogy with Equation (1),

ξ(r) = a[n(r)]ν , n(r) = [ξ(r)/a]1/ν = [r/(σa2)]1/2ν . (5)

From this result one immediately derives the power law decay for the density profile ρ(r) as follows[3, 19, 20, 26]

ρ(r) = n(r)/ξ3(r) = a−3[r/(σa2)]−(3ν−1)/2ν

≈ a−3[r/(σa2)]−0.65 (6)

Using the Flory approximation[44, 45] ν = 3/5 one would find ρ(r) ∝ r−2/3 instead.

Now the average height h of the bottle brush is esti- mated by requiring that we obtain all σN monomers per unit length in the z-direction along the axis of the bottle brush (cf. Figure 1) when we integrate ρ(r) from r = 0 to r = h,

σN =

h∫

0

N = (σa)(ν−1)/(2ν)(h/a)(ν+1)/(2ν), (8a)

4

h/a = (σa)(1−ν)/(1+ν)N2ν/(1+ν) = (σa)0.259N0.74 . (8b)

Note that the use of the Flory estimate ν = 3/5 would simply yield h ∝ σ1/4N3/4, which happens to be identical to the relation that one obtains when one partitions the cylinder of height L and radius h into disks of height σ−1, requiring hence that each chain is confined strictly into one such disk. Then each chain would form a quasi-two- dimensional self-avoiding walk formed from n′

blob = N/n′

blobs of diameter σ−1. Since we have σ−1 = an′ν again, we would conclude that the end-to-end distance R of such a quasi-two-dimensional chain is

R = σ−1(n′

blob) 3/4 = σ−1n′−3/4N3/4

= a(σa)−1+3/4νN3/4 = a(σa)1/4N3/4 . (9)

Putting then R = h, Equation (8b) results when we use there ν = 3/5. However, this similarity between Equa- tions (8b), (9) is a coincidence: in fact, the assump- tion of a quasi-two-dimensional conformation does not imply a stretching of the chain in radial direction. In fact, when we put the x-axis of our coordinate system

in the direction of the end-to-end vector ~R of the chain, we would predict that the y-component of the gyration radius scales as

Rgy = a(σa)1/4N3/4 , (10)

since for quasi-two-dimensional chains we have Rgx ∝ Rgy ∝ R, all these linear dimensions scale with the same power laws. On the other hand, if the Daoud-Cotton- like[8] picture {Figure 1a} holds, in a strict sense, one would conclude that Rgy is of the same order as the size of the last blob for r = h,

Rgy = ξ(r = h) = (h/σ)1/2

= a(σa)−ν/(1+ν)Nν/(1+ν) (11)

Clearly this prediction is very different from Equa- tion (10), even with the Flory exponent ν = 3/5 we find from Equation (11) that Rgy ∝ σ−3/8N3/8. Hence it is clear that an analysis of all three components of the gy- ration radius of a polymer chain in a bottle brush is very suitable to distinguish between the different versions of scaling concepts discussed in the literature. However, at this point we return to the geometrical

construction of the filling of a cylinder with blobs, Fig- ure 1. We explore the consequences of the obvious fact that the blobs cannot be simple spheres, when we re- quire that each blob contains monomers from a single chain only, and the available volume is densely packed with blobs touching each other. As mentioned above, ξ(r) was defined from the avail-

able surface area of a cylinder at radius r, cf. Equa- tion (4). It was argued that for each chain in the surface area Lr of such a cylinder a surface area ξ2(r) is available. However, consideration of Figure 1 shows that these sur- faces are not circles but rather ellipses, with axes fσ−1

and r/f . The blobs hence are not spheres but rather

ellipsoids, with three different axes: fσ−1 in z-direction along the cylinder axes, r/f in the y-direction tangential on the cylinder surface, normal to both the z-direction and the radial direction, and the geometric mean of these two lengths (rσ−1)1/2, in the radial x-direction. Since the physical meaning of a blob is that of a volume region in which the excluded volume interaction is not screened, this result implies that the screening of excluded volume in a bottle brush happens in a very anisotropic way: there are three different screening lengths, fσ−1 in the axial z- direction, (rσ−1)1/2 in the radial x-direction, and r/f in the third, tangential, y-direction. Of course, it remains to be shown by a more microscopic theory that such an anisotropic screening actually occurs. However, the volume of the ellipsoid with these three

axes still is given by the formula

Vellipsoid = (σ−1f)(r/f)(rσ−1)1/2 = (rσ−1)3/2 = [ξ(r)]3

(12) with ξ(r) given by Equation (4), and hence the volume of the blob has been correctly estimated by the spherical approximation. As a consequence, the estimations of the density profile ρ(r), Equation (6), and resulting brush height h, Equation (8b), remain unchanged. More care is required when we now estimate the linear

dimensions of the chain in the bottle brush. We now ori- ent the x-axis such that the xz-plane contains the center of mass of the considered chain. As Figure 1b indicates, we can estimate Rgz assuming a random walk picture in terms of blobs. When we go along the chain from the grafting site towards the outer boundary of the bottle brush, the blobs can make excursions with z = ±fσ−1, independent of r. Hence we conclude, assuming that the excursions of the nblob steps add up randomly

R2 gz =

Rgz = fσ−1√nblob . (13)

Hence we must estimate the number of blobs nblob per chain in a bottle brush. We must have

nblob =

[ξ(r)]−1dr (14)

Note from Figure 1 that we add an increment 2ξ(ri) to r when we go from the shell i to shell i+ 1 in the cylin- drical bottle brush. So the discretization of the integral in Equation (14) is equivalent to the sum. From Equa- tion (14) we then find, again ignoring factors of order unity

nblob = σ1/2h1/2 = (σa)1/(1+ν)Nν/(1+ν) , (15)

and consequently

5

With Flory exponents we hence conclude nblob ∝ σ5/8N3/8, and thus Rgz ∝ fσ−11/16N3/16. The estima- tion of Rgy is most delicate, of course, because when we consider random excursions away from the radial direc- tions, the excursions y = ±ξ(r) are non-uniform. So we have instead of Equation (13),

R2 gy =

σ−1/2h3/2 and hence

∝ σ−0.055N0.555 (18)

while the corresponding result with Flory exponents is Rgy ∝ σ−1/16N9/16. These different results for Rgx ∝ h {Equation (8b)}, Rgy {Equation (18)} and Rgz {Equation (16)} clearly reflect the anisotropic struc- ture of a chain in a bottle brush. Note that the result for Rgy according to Equation (18) is much larger than the simple Daoud-Cotton-like prediction, Equation (11), but is clearly smaller than the result of the quasi-two- dimensional picture, Equation (10). As a consistency check of our treatment, we note that

also Equation (7) can be formulated as a discrete sum over blobs

N =

[r/(σa)]1/2ν−1/2dr ,

(19) which yields Equation (8a), as it should be. Finally we discuss the crossover towards mushroom be-

havior. Physically, this must occur when the distance between grafting points along the axis, fσ−1, becomes equal to aNν . Thus we can write

h = aNνh(σaNν), (20)

where we have absorbed the extra factor f in the scaling function h(ζ). We note that Equation (8b) results from Equation (20) when we request that

h(ζ 1) ∝ ζ(1−ν)/(1+ν), (21)

and hence a smooth crossover between mushroom be- havior and radially stretched polymer conformations oc- curs for σaNν of order unity, as it should be. Analogous crossover relations can be written for the other linear di- mensions, too:

Rgz = aNνRgz(ζ), Rgz(ζ 1) ∝ ζ−(2ν+1)/(2ν+2), (22)

Rgy = aNνRgy(ζ), Rgy(ζ 1) ∝ ζ−(2ν−1)/(2ν+2), (23)

The agreement between Equation (16) and Equation (22) or Equation (18) and Equation (23), respectively, pro- vides a check on the self-consistency of our scaling argu- ments.

However, it is important to bear in mind that the blob picture of polymer brushes, as developed by Alexander,[41] Daoud and Cotton,[8] Halperin[1, 43] and many others, is a severe simplification of reality, since its basic assumptions that (i) all chains in a polymer brush are stretched in the same way, and (ii) the chain ends are all at a distance h from the grafting sites, are not true. Treatments based on the self-consistent field theory[67, 68, 69, 71, 72, 73, 74, 75, 76] and computer simulations[3, 22, 66, 70, 77, 78, 79, 80, 81, 82, 83] have shown that chain ends are not confined at the outer bound- ary of the brush, and the monomer density distribution is a nontrivial function, that cannot be described by the blob model. However, it is widely believed that the blob model yields correctly the power laws of chain linear di- mensions in terms of grafting density and chain length, so the shortcomings mentioned above affect the pre-factors in these power laws only. In this spirit, we have extended the blob model for brushes in cylindrical geometry in the present section, taking the anisotropy in the shape of the blobs into account to predict the scaling behavior of both the brush height h (which corresponds to the chain end-to-end distance R and the x-component Rgx of the gyration radius) and of the transverse gyration ra- dius components Rgy , Rgz. To our knowledge, the latter have not been considered in the previous literature.

III. Monte Carlo Methodology

We consider here the simplest lattice model of poly- mers under good solvent conditions, namely, the self- avoiding walk on the simple cubic lattice. The backbone of the bottle brush is just taken to be the z-axis of the lattice, and in order to avoid any effects due to the ends of the backbone, we choose periodic boundary conditions in the z-direction. The length of the backbone is taken to be Lb lattice spacings, and the lattice spacing henceforth is taken as one unit of length. Note that in order to avoid finite size effects Lb has to be chosen large enough so that no side chain can interact with its own “images” created by the periodic boundary condition, i.e. Rgz Lb.

We create configurations of the bottle brush poly- mers applying the pruned-enriched-Rosenbluth method (PERM).[46, 47, 48, 49, 87, 88, 89, 90] This algorithm is based on the biased chain growth algorithm of Rosen- bluth and Rosenbluth,[91] and extends it by re-sampling technique (“population control”[46]) with depth-first implementation. Similar to a recent study of star polymers[47, 48] all side chains of the bottle brush are grown simultaneously, adding one monomer to each side chain one after the other before the growth process of the first chain continues by the next step.

6

FIG. 2: Snapshot picture of a bottle brush polymer with Lb = 128 σ = 1/4, and N = 2000 on the simple cubic lattice. Note that different chains are displayed in different colors to distinguish them, and the periodic boundary condition is un- done for the sake of a better visibility in the visualization of this configuration.

When a monomer is added to a chain of length n− 1 (containing n monomers) at the nth step, one scans the neighborhood of the chain end to identify the free neigh- boring sites of the chain end, to which a monomer could be added. Out of these nfree sites available for the addi- tion of a monomer one site is chosen with the probability pn,i for the ith direction. One has the freedom to sam- ple these steps from a wide range of possible distribu- tions, e.g. pn,i = 1/nfree, if one site is chosen at random, and this additional bias is taken into account by suitable weight factors. The total weight Wn of a chain of length n with an unbiased sampling is determined recursively by Wn = Πnk=1wk = Wn−1wn. While the weight wn is gained at the nth step with a probability pn,i, one has to use wn/pn,i instead of wn. The partition sum of a chain of length n (at the nth step) is approximated as

Zn ≈ Zn ≡M−1 n

Mn∑ α=1

Wn(α), (24)

where Mn is the total number of configurations {α}, and averages of any chain property (e.g. its end-to-end dis- tance, gyration radius components, etc.) A(α) are ob- tained as

An = 1

Zn (25)

As is well-known from Ref. [84], for this original biased sampling[91] the statistical errors for large n are very hard to control. This problem is alleviated by popula- tion control.[87] One introduces two thresholds

W+ n = C+Zn, W−

n = C−Zn , (26)

where Zn is the current estimate of the partition sum, and C+ and C− are constants of order unity. The opti- mal ratio between C+ and C− is found to be C+/C− ∼ 10 in general. If Wn exceeds W+

n for the configuration α, one produces k identical copies of this configuration, re- places their weight Wn by Wn/k, and uses these copies as members of the population for the next step, where one adds a monomer to go from chain length n to n+ 1. However, if Wn < W−

n , one draws a random number η, uniformly distributed between zero and one. If η < 1/2, the configuration is eliminated from the population when one grows the chains from length n to n+1. This “prun- ing” or “enriching” step has given the PERM algorithm its name. On the other hand, if η ≥ 1/2, one keeps the configuration and replaces its weight Wn by 2Wn. In a depth-first implementation, at each time one deals with only a single configuration until a chain has been grown either to the end of reaching the maximum length or to be killed in between, and handles the copies by recursion. Since only a single configuration has to be remembered during the run, it requires much less memory.

In our implementation, we usedW+ n = ∞ andW−

n = 0 for the first configuration hitting chain length n. For the following configurations, we usedW+

n = CZn(cn/c0) and W− n = 0.15W+

n , here C = 3.0 is a positive constant, and cn is the total number of configurations of length n al- ready created during the run. The bias of growing side chains was used by giving higher probabilities in the di- rection where there are more free next neighbor sites and in the outward directions perpendicular to the backbone, where the second part of bias decreases with the length of side chains and increases with the grafting density. To- tally 105 ∼ 106 independent configurations were obtained in most cases we simulated.

Typical simulations used backbone lengths Lb = 32, 64, and 128, f = 1 (one chain per grafting site of the backbone, although occasionally also f = 2 and f = 4 were used), and grafting densities σ = 1/32, 1/16, 1/8, 1/4, 1/2 and 1. The side chain length N was varied up to N = 2000. So a typical bottle brush with Lb = 128, σ = 1/4 (i.e., nc = 32 side chains) and N = 2000 contains a total number of monomers Ntot = Lb + ncN = 64128. Figure 2 shows a snapshot configuration of such a bottle brush polymer. Note that most other simulation algo- rithms for polymers[65, 84, 85, 86] would fail to produce a large sample of well-equilibrated configurations of bottle brush polymers of this size: dynamic Monte Carlo al- gorithms using local moves involve a relaxation time (in units of Monte Carlo steps per monomer [MCS]) of or- der Nz where z = 2ν + 1 if one assumes that the side chains relax independently of each other and one ap- plies the Rouse model[92] in the good solvent regime.[85]

For N = 2000 such an estimate would imply that the time between subsequent statistically independent con- figurations is of the order of 107 MCS, which clearly is impractical. While the pivot algorithm[65] would pro- vide a significantly faster relaxation in the mushroom regime, the acceptance rate of the pivot moves quickly

7

deteriorates when the monomer density increases. This algorithm could equilibrate the outer region of the bottle brush rather efficiently, but would fail to equilibrate the chain configurations near the backbone. The configura- tional bias algorithm[86, 93] would be an interesting alter- native when the monomer density is high, but it is not expected to work for very long chains, such as N = 2000. Also, while the simple enrichment technique is useful to study both star polymers[94] and polymer brushes on flat substrates[95] it also works only for chain lengths up to about N = 100. Thus, existing Monte Carlo simulations of one-component bottle brushes under good solvent con- ditions either used the bond fluctuation model[85, 96] on the simple cubic lattice applying local moves with side chain lengths up to N = 41[30] or N = 64[36] or the pivot algorithm[65] with side chain lengths up to N = 80,[34]

but considering flexible backbone of length L = 800. An alternative approach was followed by Yethiraj[31] who studied an off-lattice tangent hard sphere model by a pivot algorithm in the continuum, for N ≤ 50. All these studies addressed the question of the overall conforma- tion of the bottle brush for a flexible backbone, and did not address in detail the conformations of the side chains. Only the total mean square radius of gyration of the side chains was estimated occasionally, obtaining[30, 36]

R2 g ∝ N1.2 or[31] R2

g ∝ N1.36 and[34] R2 g ∝ N1.4. How-

ever, due to the smallness of the side chain lengths used in these studies, as quoted above, these results have to be considered as somewhat preliminary, and also a sys- tematic study of the dependence on both N and σ was not presented. We also note that the conclusions of the quoted papers are somewhat contradictory. An interesting alternative simulation method to the

Monte Carlo study of polymeric systems is Molecular Dynamics,[85] of course. While in corresponding stud- ies of a bead-spring model of polymer chains for flat brushes[81] chain lengths N up to N = 200 were used, for chains grafted to thin cylinders[22] the three chain lengths N = 50, 100 and 150 were used. For N = 50, also four values of grafting density were studied.[22] Mu- rat and Grest[22] used these data to test the scaling pre- diction for the density profile, Equation (6), but found that ρ(r) is better compatible with ρ(r) ∝ r−0.5 rather than ρ(r) ∝ r−0.65. However, forN = 50 the range where the power law is supposed to apply is very restricted, and hence this discrepancy was not considered to be a prob- lem for the theory.[22]

Thus, we conclude that only due to the use of the PERM algorithm has it become possible to study such large bottle brush polymers as depicted in Figure 2. Nev- ertheless, as we shall see in the next section, even for such large side chain lengths one cannot yet reach the asymp- totic region where the power laws derived in the previous section are strictly valid.

IV. Monte Carlo Results for One- Component Bottle-Brush Polymers

(a)

2

1.5

1

< R

x2 > /

N

σ = 1/4 σ = 1/8 σ = 1/16 σ = 1/32 σ = 1/64 σ = 1/128

(b)

0.1

0.095

0.09

0.085

< R

y2 > /

N

σ = 1/4 σ = 1/8 σ = 1/16 σ = 1/32 σ = 1/64 σ = 1/128

(c)

0.6

0.5

0.4

0.3

< R

z2 > /

N

σ = 1/128 σ = 1/64 σ = 1/32 σ = 1/16 σ = 1/8 σ = 1/4

FIG. 3: Log-log plot of the mean square end-to-end distance components R2

x (a), R2

y (b), and R2

z (c) versus side chain length N , for various choices of the grafting density σ as indi- cated. All data refer to f = 1 (one chain per possible grafting site) and N > 5. Note that the x-direction for every chain is the normal direction from its center of mass position to the bottle brush backbone. All data are for Lb = 128. The chain mean square linear dimensions are all normalized by N2ν .

In Figures 3 and 4, we present our data for the mean square end-to-end radii and gyration radii components of the side chains. Note that for each chain configuration a separate local coordinate system for the analysis of the chain configuration needs to be used; while the z-axis is always oriented simply along the backbone, the x-axis is oriented perpendicular to the z-axis and goes through the center of mass of the chain in this particular config- uration. The y-axis then also is fixed simply from the requirement that it is perpendicular to both the x- and z-axes.

For a polymer mushroom (which is obtained if the

8

(a)

0.3

0.2

0.1

< R

/ N

2ν

N

σ = 1/4 σ = 1/8 σ = 1/16 σ = 1/32 σ = 1/64 σ = 1/128

(b)

0.04

0.038

< R

/ N

2ν

N

σ = 1/4 σ = 1/8 σ = 1/16 σ = 1/32 σ = 1/64 σ = 1/128

(c) 0.13

< R

/ N

2ν

N

σ = 1/128 σ = 1/64 σ = 1/32 σ = 1/16 σ = 1/8 σ = 1/4

FIG. 4: Log-log plot of the mean square gyration radius com- ponents R2

gx (a), R2

gy (b), and R2

gz (c), versus side chain length N . Only data for N > 10 are included. All data are for f = 1, Lb = 128, and various choices of σ. All chain mean square linear dimensions are normalized by N2ν with ν = ν3 ≈ 0.588.

grafting density σ is sufficiently small) we expect that all chain linear dimensions scale as Nν , for sufficiently long chains. Therefore we have normalized all mean square linear dimensions in Figures 3 and 4 by a factor N2ν , using the theoretical value[64, 65] ν = 0.588. However, as we see from Figures 3, 4 in the range 10 ≤ N ≤ 103 dis- played there, even for the smallest σ presented, where a single side chain is simulated, the shown ratios are not constant. This fact indicates that corrections to scaling[64, 65] should not be disregarded, and this prob- lem clearly complicates the test of the scaling predic- tions derived above. For the largest value of σ included (σ = 1/4), the irregular behavior of some of the data (Figure 3b,c, Figure 4b) indicate a deterioration of sta-

(a) 2.2

(R 2 x+

R 2 y)

(R 2 x+

R 2 y)

⊥ = R2

y divided by N2ν

vs. ζ = σNν , including all data for N > 5, and three choices of Lb as indicated (a), or alternatively removing data affected by the finite size of the backbone length via the periodic bound- ary condition (b). The slope indicated in (b) by the dotted straight line corresponds to the scaling estimate from Equa- tion (21), 2(1− ν)/(1 + ν) ≈ 0.519.

tistical accuracy. This problem gets worse for increasing number of side chains nc.

A further complication is due to the residual finite size effect. Figure 5 shows a plot of R2

⊥ = R2

x + R2 y vs. the

scaling variable ζ = σNν . One can recognize that for small Lb but large N and not too large σ systematic deviations from scaling occur (Figure 5a), which simply arise from the fact that an additional scaling variable (related to R2

z1/2/Lb) comes into play when R2 z1/2 no

longer is negligibly smaller than Lb. While for real bot- tle brush polymers with stiff backbone effects due to the finite lengths of the backbone are physically meaningful and hence of interest, the situation is different in our simulation due to the use of periodic boundary condi- tions. The choice of periodic boundary conditions is mo- tivated by the desire to study the characteristic structure in a bottle brush polymer far away from the backbone ends, not affected by any finite size effects. However, if R2

gz1/2 becomes comparable to Lb, each chain interacts with its own periodic images, and this is an unphysical, undesirable, finite size effect. Therefore in Figure 5b, the data affected by such finite size effects are not included. One finds a reasonable data collapse of the scaled mean square end-to-end distance when one plots the data ver- sus the scaling variable ζ = σNν . These results consti-

9

(a)

0.5

0.1

< R

gx2 > /

N 2ν

ζ = σNν

slope = 0.519

σ = 1/128 σ = 1/64 σ = 1/32 σ = 1/16 σ = 1/8 σ = 1/4

(b)

0.5

0.1

< R

gy2 > /

N 2ν

ζ = σNν

slope = -0.111

σ = 1/128 σ = 1/64 σ = 1/32 σ = 1/16 σ = 1/8 σ = 1/4

(c)

0.5

0.1

< R

gz2 > /

N 2ν

ζ = σNν

slope = -1.370

σ = 1/128 σ = 1/64 σ = 1/32 σ = 1/16 σ = 1/8 σ = 1/4

FIG. 6: Log-log plot of R2

gx/N2ν (a), R2

gy/N2ν (b) and R2

gz/N2ν (c) versus the scaling variable ζ = σNν , using the data in Figure 4 but for N > 50. The slopes indicated by dashed straight lines illustrate the scaling estimates from Equation (21), 2(1 − ν)/(1 + ν) ≈ 0.519 (a), from Equa- tion (23), −(2ν − 1)/(ν + 1) ≈ −0.111 (b), and from Equa- tion (22), −(2ν + 1))/(ν + 1) ≈ −1.370 (c).

tute the first comprehensive test of the scaling relations for bottle brush polymers, Equations (21) - (23), and the consistency between the data and the proposed scaling structure in terms of the variable ζ is indeed very grati- fying. On the other hand, it is also evident from Figures 5 and 6 that only a mild stretching of the side chains away from the backbone is observed, and in this region one is still far away from the region of strong stretching, where the simple power laws Equations (8b), (18) and (16) ap- ply. Obviously, the crossover from the simple mushroom behavior (observed for ζ = σNν 1) to the strongly stretched bottle brush (observed for ζ 1) takes at least one decade of the scaling variable ζ. There is a rather

(a)

0.001

0.01

0.1

< R

N

σ = 1 σ = 1/3 σ = 1/7 σ = 1/15 σ = 1/31 σ = 1/63

(b)

0.001

0.01

0.1

< R

N

σ = 1 σ = 1/3 σ = 1/7 σ = 1/15 σ = 1/31 σ = 1/63

(c)

0.01

0.1

1

10

100

1000

< R

σ = 1/63 σ = 1/31 σ = 1/15 σ = 1/7 σ = 1/3

FIG. 7: Log-log plot of the mean-square gyration radius com- ponents R2

gx,slit/N2ν2 (a), R2

gy,slit/N2ν2 (b) and R2

gz,slit (c) versus side chain length N with ν2 = 3/4. As in Fig- ure 4, only data for N > 5 are included. Various choices of σ are included. Note that the walls of the slit are located at z = ±(σ−1 + 1)/2 and are strictly repulsive hard walls. One chain end is fixed at the x-axis at z = 0, and since the x-axis represents the backbone if this polymer in a slit is taken as a model of a disk-shaped section of a bottle brush, all sites of the x-axis are excluded from occupation of the monomers of the (side) chain as well.

gradual and smooth crossover rather than a kink-like be- havior of the scaling function. While in the x-component at least near ζ = 10 a weak onset of stretching can be recognized, hardly any evidence for the contraction of the y and z-components is seen.

In order to test what one would expect if the picture of the chains as quasi-two-dimensional self-avoiding walks were correct, we have also studied single chains grafted to a straight backbone of length σ, σ = 1, 1/3, 1/5, . . .1/63

10

(a)

0.01

0.1

1

< R

(b)

0.01

0.1

1

< R

(c)

1e-05

1e-04

0.001

0.01

0.1

1

< R

FIG. 8: Log-log plot of Rgx,slit/N2ν (a), R2

gy,slit/N2ν , and

R2

gzslit/N2ν (c) versus the scaling variable ζ = σNν . Only data for N > 10 are included. The slopes indicated by dashed straight lines illustrate the scaling exponent implied by Equa- tion (27), namely 3/2ν − 2 (a,b) and −2 (c), respectively. In (c) σ−1 is replaced by σ−1 + 1 to remove a finite-size effect.

which are confined between two parallel repulsive infinite walls. The grafting site of the chains was chosen at the site located symmetrically between the confining walls in the slit {if the grafting site is chosen to be the origin of the coordinate system, the confining hard walls occur at z = ±(σ−1 + 1)/2}. Figure 7 gives log-log plots of the gyration radii components of such chains confined to such disk-like slits, which we denote as Rgα, slit, α = x, y and z, in order to distinguish then from the actual gyration radii components of the side chains in a bottle brush polymer. One can clearly see that R2

gx,slit, R2 gy,slit

scale as N2ν2 = N3/2 for large N , as it must be. These data are very similar to data for chains confined between

(a)

1

σ = 1/63 σ = 1/31 σ = 1/15 σ = 1/7 σ = 1/3

(b)

0.1

1

σ = 1/63 σ = 1/31 σ = 1/15 σ = 1/7 σ = 1/3

(c)

1

10

100

1000

σ = 1/3 σ = 1/7 σ = 1/15 σ = 1/31 σ = 1/63

FIG. 9: Log-log plot of R2

gx/R2

gz/R2

gz,slit versus N , for values of σ strictly cor- responding to each other, as indicated.

repulsive walls without a grafting to a piece of a rigid backbone,[97] of course. In the corresponding scaling plot (Figure 8) one can see that both R2

gx,slit and R 2 gy,slit have

the simple crossover scaling behavior[45, 98]

R2 gx,slit = N2ν fx(σN

ν) (27)

with fx(ζ) ∝ fy(ζ) ∝ ζ2(ν2−ν)/ν with ν2 = 3/4, as ex-

pected, and seen in related previous work.[97, 99] Obvi- ously, although we use in Figures 7 and 8 the same range of N and σ as in Figures 4 and 6, the behavior is rather different. As expected from our scaling analysis pre- sented above, the confinement that a chain experiences in a bottle brush due to the presence of the other chains is much weaker than the confinement of a chain in the equivalent disk-like sector between confining walls. This

11

(a)

1e-04

0.001

0.01

0.1

1

slope = -0.65

σ = 1/128 σ = 1/64 σ = 1/32 σ = 1/16 σ = 1/8 σ = 1/4

(b)

1e-04

0.001

0.01

0.1

1

slope = -0.65

σ = 1/128 σ = 1/64 σ = 1/32 σ = 1/16 σ = 1/8 σ = 1/4

(c)

1e-04

0.001

0.01

0.1

1

slope = -0.65

σ = 1/128 σ = 1/64 σ = 1/32 σ = 1/16 σ = 1/8 σ = 1/4

FIG. 10: Radial distribution function ρ(r) plotted vs. r, for N = 500 (a), N = 1000 (b), and N = 1500 (c), for various choices of σ, as indicated. Note that due to the discreteness of the lattice, the number N(r) of monomers in the interval [r, r+dr] is not normalized by the factor πr that applies in the continuum limit, but by the number Nr of lattice sites (x,y) satisfying the constraint r2 = x2 + y2, i.e.

P

r N(r) = N and

ρ(r) = N(r)/Nr . All data refer to Lb = 128 and f = 1.

fact is demonstrated very directly in Figure 9, where the ratios R2

gα/R2 gα,slit are plotted vs. N for the corre-

sponding values of σ. If the hypothesis of quasi-two di- mensional confinement were valid, we would expect these ratios to be constants. Obviously, this is not the case.

As a final point of this section, we discuss the distri- bution of monomers (Figures 10 and 11) and chain ends (Figures 12 and 13) in the simulated model for the bottle brush polymer. Unlike corresponding radial density dis- tributions for the off-lattice bead-spring model of Murat and Grest,[22] where for small distances close to the back- bone a kind of “layering” was observed, we see a rather

(a)

0

5

10

15

20

< ρ(

z) >

z

σ = 1/128 σ = 1/64 σ = 1/32 σ = 1/16 σ = 1/8

(b)

0

5

10

15

20

25

< ρ(

z) >

z

σ = 1/128 σ = 1/64 σ = 1/32 σ = 1/16 σ = 1/8

(c)

0

5

10

15

20

25

30

< ρ(

z) >

z

σ = 1/128 σ = 1/64 σ = 1/32 σ = 1/16 σ = 1/8

FIG. 11: Density distribution function ρ(z) plotted vs. the coordinate z along the backbones, for N = 500 (a), N = 1000 (b), and N = 1500 (c), and various choices of σ, as indicated. This distribution is normalized by choosing

P

z ρ(z) = 1

smooth behavior also for small distances (Figure 10). For larger distances, the behavior is qualitatively very sim- ilar. Again we fail to provide a clear-cut evidence for the predicted power law decay, Equation (6). Note, how- ever, that this power law is supposed to hold only in the strong stretching limit, where Equation (8b) is ob- servable (which we do not verify either), and in addition the stringent condition 1 r h needs to be obeyed, to have this power law. Although our simulations en- compass much longer chains than every previous work on bottle brushes, we clearly fail to satisfy this double inequality. Turning to the distribution along the backbone (Fig-

ure 11), the periodicity due to the strictly periodic spac- ing of grafting sites is clearly visible. If desired, one could also study a random distribution of grafting sites along

12

(a)

0

2

4

6

8

< ρ e

σ = 1/128 σ = 1/64 σ = 1/32 σ = 1/16 σ = 1/8

(b)

4

6

8

10

12

< ρ e

σ = 1/128 σ = 1/64 σ = 1/32 σ = 1/16 σ = 1/8

(c)

10

12

14

< ρ e

σ = 1/128 σ = 1/64 σ = 1/32 σ = 1/16 σ = 1/8

FIG. 12: Density distributions of chain ends ρe(z) plotted vs. z, for the same choice of parameters as in Figure 11.

the backbone, of course, but we have restricted attention to the simplest case of a regular arrangement of grafting sites only. The distribution of chain ends ρ(z) exhibits an analogous periodicity for small values of σ only, while ρe(z) is approximately constant (Figure 12) for larger values of σ.

Most interesting is the radial distribution of chain ends (Figure 13). One can see an increasing depression of ρe(r) for small r when σ increases. Again these data are similar to the off-lattice results of Murat and Grest.[22] In no case do we see the “dead zone” predicted by the self-consistent field theory in the strong stretching limit,[21, 24] however.

V. Phase Separation in Two-Component Bottle Brushes: Theoretical Background

(a)

0

0.02

0.04

0.06

0.08

0.1

< ρ e

nd (r

r

σ = 1/128 σ = 1/64 σ = 1/32 σ = 1/16 σ = 1/8 σ = 1/4

(b)

0

0.02

0.04

0.06

0.08

0.1

< ρ e

nd (r

r

σ = 1/128 σ = 1/64 σ = 1/32 σ = 1/16 σ = 1/8 σ = 1/4

(c)

0

0.02

0.04

0.06

0.08

0.1

< ρ e

nd (r

r

σ = 1/128 σ = 1/64 σ = 1/32 σ = 1/16 σ = 1/8 σ = 1/4

FIG. 13: Radial density distribution of chain ends ρe(r) plot- ted vs. r, for the same choice of parameters as in Figures 10- 12.

We still consider a bottle brush polymer with a strictly rigid straight backbone, where at regularly distributed grafting sites (grafting density σ) side chains of length N are attached, but now we assume that there are two chemically different monomeric species, A and B, com- posing these side chains with NA = NB = N . These systems have found recent attention, suggesting the pos- sibility of intramolecular phase separation. [56, 57, 58] In a binary system pairwise interaction energies AA, AB, and BB are expected, and consequently phase separation between A and B could be driven by the Flory-Huggins parameter

χ = zc/kBT, = AB − (AA + BB)/2 (28)

where zc is the coordination number of the lattice, like in the Flory-Huggins lattice model of phase separation in

13

y

FIG. 14: Schematic description of perfect phase separation of side chains in a cylindrical binary (A,B) bottle brush poly- mer into a “Janus cylinder” structure, where the A-chains occupy the lower hemicylinder and the B-chains occupy the upper hemicylinder. The interface between B-rich and A-rich phases is assumed to be oriented in the yz-plane. The figure indicates the characterization of this order in terms of a local order parameter, namely the vector ~ψ(z) oriented normal to the interface at every grafting site. The absolute value of this vector characterizes a suitable average of the local phase sep- aration in a disk of the cylinder located at z (see text). For

perfect order | ~ψ(z) | = 1 and ~ψ(z) is oriented along the same axis for the whole bottle brush polymer.

a binary polymer blend. [44, 45, 50, 51, 52] However, since the side chains are grafted to the backbone, only in- tramolecular phase separation is possible here. Actu- ally, the energy parameter suffices for dense polymer blends or dense block copolymer melts, where no solvent is present. [44, 45, 50, 51, 52] For the problem of intramolec- ular phase separation in a bottle brush, the solvent can- not be disregarded and hence the enthalpy of mixing rather is written as.[52, 56]

Emix/kBT =

∫ dV

+ χABφA(~r)φB(~r)], (29)

where v is the volume per monomer, φA(~r), φB(~r) and φS(~r) are the local volume fractions of monomers of types A and B, and the solvent density, respectively, and three pairwise interaction parameters χAS , χBS, and χAB en- ter. The latter χAB corresponds to the χ-parameter writ- ten in Equation (28), while the former two control the solvent quality for polymers A and B, respectively. Of course, using the incompressibility condition

φA(~r) + φB(~r) + φS(~r) = 1 (30)

the solvent density can be eliminated from the problem (but one should keep in mind that in the free energy density there is an entropy of mixing term φS(~r) lnφS(~r) present [56]). In the framework of the lattice model stud- ied here, v ≡ 1 and solvent molecules are only implicitly considered, identifying them with vacant sites. For sim- plicity, the following discussion considers only the most symmetric case, where χAS = χBS , and the numbers of A chains and B chains are equal. Stepanyan et al. [56] used Equations (29) and (30),

as the starting point of a self-consistent field calcula-

tion, adding conformational free energy contributions ac- counting for the entropy associated with the stretching of Gaussian chains. It is found that when χAB exceeds a critical value χ∗

AB, intramolecular phase separation of “Janus cylinder”-type occurs (Figure 14). Then an in- terface is formed, containing the backbone of the bottle brush, such that there is an excess of A-monomers below the interface and an excess of B-monomers above the in- terface (or vice versa). Assuming that at the position z of the backbone the interface is oriented in x-direction, we can describe this Janus-type phase separation in terms of an one-dimensional order parameter density

ψ(z) = (n+ B−n+

B are the numbers of A(B) monomers

in the interval [z, z + dz] with x > 0(n+ A, n

+ B) and x <

A, n −

B), respectively. Since we shall see below that the orientation of the interface is an important degree of freedom, we may consider ψ(z) as the absolute value of

a vector order parameter ~ψ(z), and the direction of ~ψ(z) is defined such that ψ(z) takes a maximum. However, Stepanyan et al. [56] did not consider the possibility of an inhomogeneity along the z-axis, and they also did not derive how the order parameter depends on the parame- ters N , σ, and the various χ parameters of the problem {Equation (29)}. Stepanyan et al.[56] also assume that the distribution of chain ends is a delta function at the radius (or “height” h) respectively) of the bottle brush, where h is given by h/a = (σa)1/4N3/4 in the good sol- vent regime. They then find that phase separation occurs for

χ∗

AB ∝ 1/ √ N, (32)

but argue that this result holds only for a “marginal sol- vent” rather than a good solvent, due to the mean-field approximation used which neglects that inside a blob all binary contacts are avoided, estimating the number of contacts simply proportional to the product φAφB , cf. Equation (29), and neglecting the correlations due to excluded volume. The regime of marginal solvents is reached near the θ-point (which occurs for 1 − 2χAS = 1− 2χBS = 0), and requires that [56]

0 < 1− 2χAS < N−1/3 (33)

where again prefactors of order unity are omitted. Stepanyan et al. [56] extend Equation (32) by a simple

scaling-type argument, stating that the transition from the mixed state to the separated state occurs when the energy of the A-B contacts per side chain, E, is of the order of kBT . They estimate this energy as

E/kBT ≈ Np(φ)χAB , (34)

where p(φ) is the probability of the A-B contact, which depends on the average volume fraction φ of the monomers inside the brush. According to the mean field

14

A

A

B

B

y

FIG. 15: Same as Figure 14, but allowing for a long wave-

length variation of the vector ~ψ(z) characterizing the local interface orientation in the Janus cylinder.

cT

ξ

R

T

0

FIG. 16: Schematic sketch of the temperature dependence of the correlation length ξ of the ferromagnetic XY-model in a cylinder of radius R.

theory, p(φ) ∝ φ, where φ = N/h2, h being the ra- dius of the cylindrical brush. Using h ∝ N3/4 (Equa- tion (8b)) one finds p(φ) ∝ N−1/2 and using this result in Equation (34) implies E/kBT ∝ N1/2χAB, and from E/kBT = 1 we recover Equation (32). The merit of this simple argument is that it is readily

extended to other cases: e.g., for a θ-solvent, we have[18]

h ∝ N2/3 and hence p(φ) ∝ N−1/3, yielding [56]

χ∗

AB ∝ N−2/3 , θ − solvent. (35)

For the poor solvent case, the bottle brush should col- lapse to a cylinder densely filled with monomers, and hence h ∝ N1/2, φ = 1, and thus

χ∗

AB ∝ N−1 , poor solvent. (36)

Note that Equation (36) is the same relation as for a dense bulk polymer blend or block copolymer melt, respectively.[44, 45, 50, 51, 52]

The situation is more subtle in the good solvent case, however, since there the probability of contact is no longer given by the mean field result p(φ) ∝ φ but rather by [45]

p(φ) ∝ φ5/4 ∝ N−5/8 , (37)

where the Flory approximation ν = 3/5 was again used, with φ ∝ N−1/2 when h ∝ N3/4. Equations (34) and

(37) now imply

AB ∝ N−3/8 , good solvent (38)

However, these crude estimates do not suffice to prove that for χAB > χ∗

AB true long range order of this “Janus

cylinder” type (Figure 14) is established. Hsu et al.[58]

suggested that there is also the need to consider varia-

tions of the direction of the order parameter ~ψ(z) along the z-direction (Figure 15). It was argued that for any finite side chain length N also the cylinder radius (or brush “height”) h is finite, and hence the system is one-dimensional. In one-dimensional systems with short range interactions at nonzero temperatures no long range order is possible.[100, 101] The situation depicted in Fig- ure 15 is reminiscent of the one-dimensional XY-model of a chain of spins on a one-dimensional lattice where each spin at site i is described by an angle i in the xy- plane, with 0 ≤ i ≤ 2π, and where neighboring spins are coupled. This coupling is described by the Hamiltonian

H = −J ∑ i

~Si+1 · ~Si (39)

when ~Si = (cosi, sini) is a unit vector in the xy-plane. While mean field theory predicts that ferromagnetic or- der occurs along the chain, for ferromagnetic exchange J > 0 and temperatures T less than the critical tem- perature TMF

c which is of the order of J/kB, the exact solution of this model, Equation (39), shows[100, 101] that Tc = 0, since ferromagnetic long range order is unstable against long wavelength fluctuations. One can show that the spin-spin correlation function for large z = a(j − i) decays to zero exponentially fast,

~Si · ~Sj ∝ exp[−z/ξ], z → ∞ (40)

where a is the lattice spacing of this spin chain. The correlation length ξ gradually grows as the temperature is lowered,

ξ = 2a(J/kBT ) (41)

Equation (41) is at variance with mean field theory, which rather would predict[100] (the index MF stands for “mean field” throughout)

ξMF ∝ (T/TMF c − 1)−νMF , νMF = 1/2 . (42)

This critical divergence at a nonzero critical tempera- ture TMF

c is completely washed out by the fluctuations: rather than diverging at TMF

c , the actual correlation length ξ {Equation (41)} at TMF

c still is only of the order of the lattice spacing. This consideration can be generalized to spin sys-

tems on lattices which have a large but finite size in (d − 1) dimensions and are infinite in one space dimen- sions only.[102, 103] E.g., when we consider an infinitely

15

long cylinder of cross section πR2 we expect that Equa- tions (41), (42) are replaced by the finite size scaling relation [104, 105]

ξ = ξ∞ ξ(R/ξ∞) , ξ(ζ 1) = 1 , ξ(ζ 1) ∝ ζ , (43)

where ξ∞ is the correlation length of the XY model on a lattice which is infinitely large in all d = 3 directions of space.

ξ∞ ∝ (T/Tc − 1)−ν , (44)

where again kBTc ∝ J (but with a smaller constant of proportionality than that in the relation kBT

MF c ∝ J),

and ν is the correlation length exponent of the XY model (ν ≈ 0.67).[106] Equation (43) describes a smooth crossover of the ferromagnetic correlation length describ- ing spin correlations along the axis of the cylinder from bulk, Equation (44), to a quasi-one-dimensional varia- tion. For T Tc the correlation length resembles Equa- tion (41), since[102, 103]

ξ = 2πΓ(T )R2/kBT ≈ 2π(R2/a)(J/kBT ), T → 0. (45)

the “helicity modulus” (also called “spin wave stiffness”) Γ(T ) is of order J for T → 0 and shows a critical vanish- ing as T → Tc from below, in the thermodynamic limit R → ∞. However, for finite R there is a finite size round- ing of this singularity of Γ(T → Tc), such that Γ(T = Tc) is of order 1/R, and hence a smooth crossover to Equa- tion (43) occurs near Tc. Figure 16 gives a qualitative account of this behavior. For more details of this finite size crossover we refer to the literature.[102, 103] But we suggest a qualitatively similar behavior for the domain size ξ of segregated A-rich and B-rich domains in binary bottle brush polymers. So, when we study the correla- tion function of the order parameter considered in Equa- tion (31)

Gψ(z) = ~ψ(z′) · ~ψ(z′ + z) ∝ exp(−z/ξψ) (46)

we expect that the correlation length ξψ describing the lo- cal phase separation in the direction along the backbone of the bottle brush polymer remains of order unity as long as χ−1

AB exceeds χ∗ −1 AB distinctly. For χAB near χ∗

AB we expect that ξψ becomes of order h, the radius of the bottle brush. For χAB χ∗

AB, we expect ξψ ∝ h2χAB, by analogy with Equation (45). Unfortunately, the test of those predictions even in the poor solvent case where χ∗ −1 AB is largest, is rather difficult, since the prefactor in

the relation χ∗ AB ∝ 1/N is unknown.

VI. Monte Carlo Results for Binary Bottle Brush Polymers

We use the same lattice model as considered before in our Monte Carlo study of the chain conformations of

one-component bottle brush polymers, but now in the construction of the weights Wn(α) we have to take into account that the partition function now is

Z = ∑ α

qmAA+mBBqmAB

AB (47)

with (remember that we restrict attention to the choice AA = BB)

q = exp(−AA/kBT ), qAB = exp(−AB/kBT ) . (48)

In Equation (47) the numbers of non-bonded occupied nearest-neighbor monomer pairs AA, BB and AB are de- noted as mAA,mBB and mAB, respectively. Note that the sum in Equation (47) extends over all possible con- figurations {α} of the bottle brush polymer. The choice q = qAB = 1 corresponds to the previously studied one- component bottle brush under good solvent conditions, while the choice q = qAB > 1 corresponds to variable solvent quality for the one-component brush (note that q = qAB means χ = 0, Equation (28), and also χAB which is proportional to χ then vanishes: this means there is no chemical incompatibility between A and B any longer, no physical difference between A and B ex- ists any more). From previous work on single chains[46]

we know that the θ-point occurs for qθ = 1.3087. There- fore we varied q in the range 1 ≤ q ≤ 1.5; q = 1.5 hence falls in the regime of poor solvent quality already. Of course, in order to have rather compact configurations of cylindrical bottle brushes a choice of much larger q would be desirable. However, the efficiency of the PERM algo- rithm quickly deteriorates with increasing q: for q = 1.5 we encounter already for rather small values of the side chain length N such as N = 18 and a backbone length of Lb = 64 huge statistical fluctuations. The total size of the bottle brush polymer under poor solvent condi- tions reached here, Ntot = NσLb + Lb = 1216, is al- most two orders of magnitude smaller than the maxi- mal size studied under good solvent conditions! How- ever, all known simulation algorithms for polymers suffer from difficulties of equilibration in the limit of very dense configurations. [84, 85, 86]

Since we are mostly interested in the high grafting limit (σ = 1, so the number of side chains nc = σLb = Lb) in the PERM algorithm where all side chains grow simultaneously we use a bias factor such that side chains are grown with higher probability in the direc- tions perpendicular to the backbone. This additional bias (which is not present in the standard Rosenbluth [91]

and PERM[46] methods) must be taken into account by suitable weight factors. About 106 independent configu- rations were typically generated. Figures 17 - 19 now show typical results for the good

solvent case (q = 1) but varying the parameter qAB con- trolling the chemical incompatibility. The visual inspec- tion of the configurations (Figure 17) reveals little in- fluence of qAB, however, and this observation is corrob- orated by the more quantitative analysis: the average

16

(a)

(b)

(c)

FIG. 17: Snapshot pictures of bottle brush configurations for Lb = 64, q = 1, N = 18, σ = 1 and three choices of qAB , qAB = 1.0 (a), qAB = 0.4 (b) and qAB = 0.1 (c). Monomers A, monomers B, and a straight rigid backbone are shown in black, light gray, and white colors, respectively.

(a)

0

0.03

0.06

0.09

0.12

0.15

< m

C v

N = 6

N = 12

N = 18

FIG. 18: (a) Average number of AB pairs per monomer mAB/(Nnc) plotted vs. qAB for side chain lengths N = 6, 12, and 18. All data refer to σ = 1, Lb = 64. (b) Specific heat per monomer, cv/(Nnc) plotted vs. qAB for N = 6, 12 and 18.

(a)

0

0.1

0.2

0.3

0.4

(< R

x2 > +

< R

y2 > )

qAB=0.1

qAB=0.5

qAB=1.0

FIG. 19: (a) Radial density distribution ρ(r) plotted vs. r for Lb = 64, N = 18, q = 1, σ = 1, f = 1 and various qAB . (b) Normalized transverse mean square end-to-end distance (R2

x + R2

y)/N2ν plotted vs. N , for Lb = 64, q = 1, σ = 1, f = 1, and three choices of qAB as shown.

17

x

y

3

n

FIG. 20: Vectors ~Rα cm(n) from the grafting site n to the xy-

component of the center of mass of the respective chain, and corresponding unit vectors (denoted by arrows). For a per- fectly phase separated structure with the interface between A and B being the yz plane, for α = A all unit vectors point along the negative x-axis and for α = B all unit vectors point along the positive x-axis.

(a)

0

0.1

0.2

n

qAB = 0.1 qAB = 0.2 qAB = 0.3 qAB = 0.4 qAB = 0.5 qAB = 0.6

(b)

0

0.1

0.2

0.3

n

qAB = 0.1 qAB = 0.2 qAB = 0.3 qAB = 0.4 qAB = 0.5 qAB = 0.6

(c)

0

0.1

0.2

0.3

C n

n

qAB = 0.1 qAB = 0.2 qAB = 0.3 qAB = 0.4 qAB = 0.5 qAB = 0.6

FIG. 21: Correlation function Cn measuring local “Janus cylinder”-type phase separation plotted versus n, for N = 6 (a), 12 (b), and 18 (c). Various choices of qAB are included, as indicated in the figure. Curves show fits to Equation (50). All data refer to good solvent conditions (q = 1), and Lb = 64, σ = 1, f = 1.

(a)

0

0.05

0.1

0.15

0.2

0.25

0.3

P (θ

θ / π

qAB = 0.1 qAB = 0.2 qAB = 0.4 qAB = 0.6 qAB = 0.8 qAB = 1.0

(b)

0

0.05

0.1

0.15

0.2

0.25

0.3

P (θ

θ / π

qAB = 0.1 qAB = 0.2 qAB = 0.4 qAB = 0.6 qAB = 0.8 qAB = 1.0

FIG. 22: Distribution P (θ) of the angle θ between the vectors towards the centers of mass of subsequent (unlike) side chains plotted vs. θ/π, for N = 12 (a) and N = 18 (b). Various choices of qAB are included, as indicated.

number of A-B pairs per monomer is extremely small (Figure 18a) even for qAB = 1, and hence not much enthalpy could be won if A-chains and B-chains avoid each other: due to the excluded volume interaction, very few nearest neighbor contacts between any non-bonded monomers occur in our bottle brush model. For N = 18 and qAB = 1 the total number of AB contacts per chain is only about 1.4, and increases with increasing N only very slowly. So for the range of side chain lengths ac- cessible in our work, no phase separation should be ex- pected. In the specific heat one does see a weak peak near 0.2 ≤ qAB ≤ 0.4, but the height of this peak decreases very strongly with increasing N . Furthermore does nei- ther the peak position shift with increasing N (as one would expect from Equation (38), if this peak would be a rounded precursor of the phase transition that should occur at χ∗

AB in the limit N → ∞) nor does the peak width decrease with increasing N . Thus, it is clear that this peak is not an indicator of a “Janus-cylinder”-type phase separation in the bottle brush: rather we interpret it as a Schottky-type anomaly, expected from the fact that in our model of alternatingly grafted A-and B-chains at a straight line backbone with coordinates (0, 0, z) in the immediate environment of the backbone (e.g. at lat- tice sites (x, y, z) = (±1, 0, z) or (0,±1, z)) there is a nonzero a-priori probability of 1/4 that between the first monomer of the chain grafted at z and the first monomer of the chain grafted at z + 1 a nearest-neighbor contact

18

(a)

0

0.01

0.02

0.03

0.04

C v

(b)

0

0.1

0.2

0.3

0.4

qAB = 0.1

qAB = 0.3

qAB = 0.5

FIG. 23: (a) Specific heat per monomer, CN/(Nnc), plotted vs. qAB for N = 6, 12, and 18 for σ = 1, Lb = 64, and q = 1.3087 (a Theta solvent). (b) Radial density distribution ρ(r) plotted vs. r for Lb = 64, N = 18, q = 1.3087, σ = 1, f = 1, and three choices of qAB .

occurs. The finite energy from this local contacts near the backbone gives rise to the peak in the specific heat. Also the radial density profile (Figure 19a) shows lit-

tle effects of varying qAB , and there is also no effect in the gyration radius component R2

g⊥ = R2 gx + R2

gy of the side chains, although a weak increase occurs in the corresponding component of the end-to-end distance (Figure 19b). In the latter figure, one can see for small N an even-odd oscillation, but this lattice effect clearly has died out for N > 10. In order to test for correlations measuring local phase

separation along the backbone, Equation (46) is some- what cumbersome to implement numerically, since for

each z one has to find the direction of ~ψ(z) from the

condition that |~ψ(z)| is maximal (cf. Equation (31)). A simpler and similar correlation function has been defined from the vectors pointing from the grafting site i to the center of mass of the respective side chains. Projecting this vector into the xy-plane and defining an unit vector ~Sαi (α = A or B) along this projection (Figure 20) we define a correlation function Cn as follows

Cn ≡ [~SAi · ~SAi+n+ ~SBi+1 · ~SBi+1+n]/2 . (49)

Here we have explicitly incorporated the alternating grafting ABAB... of side chains along the backbone. The average . . . in Equation (49) includes an averaging over

(a)

1

1.2

1.4

1.6

(< R

x2 > +

< R

y2 > /

N

N

P (θ

FIG. 24: (a) Normalized transverse mean square end-to-end distance (< R2

x > + < R2

y >)/N plotted vs. N , for Lb = 64, σ = 1, f = 1, and q = 1.3087 (Theta solvent). Three choices of qAB are included. (b) Distribution P (θ) of the angle be- tween the vectors towards the centers of mass of subsequent (unlike) side chains plotted vs. θ/π, for N = 18, other param- eters as in (a).

all sites {i} on which A chains are grafted, in order to im- prove the statistics. If perfect long range order occurs, as implied in Figure 20, we clearly have Cn = 1 independent of n, while for the case of short range order, we expect Cn ∝ exp(−n/ξ). Actually, considering the fact that we use a periodic boundary condition, we have analyzed our numerical data in terms of the ansatz

Cn ∝ {exp(−n/ξ) + exp[−(Lb − n)/ξ]} . (50)

Figure 21 shows our data for Cn for the three choices of N : indeed we recognize that Cn decays to zero with in- creasing n, but the increase does get slower with increas- ing side chain length N . The scale of this correlation effect clearly increases with decreasing qAB. While for N = 6 the correlation length ξ hardly depends on qAB, for large N a slight increase of ξ with decreasing qAB is suggested.

In an earlier simulation study of phase separation in binary bottle brushes, [57] it was suggested to quantify the degree of separation by considering the distribution of the polar angle i from the axis to monomer . Defining a variable σA , which is σA = 1 if monomer is of type A and zero otherwise, and similarly σB , de Jong and ten

19

(a)

0

0.1

0.2

0.3

0.4

n

qAB = 0.1 qAB = 0.2 qAB = 0.3 qAB = 0.4 qAB = 0.5 qAB = 0.6

(b)

0

0.1

0.2

0.3

0.4

0.5

n

qAB = 0.1 qAB = 0.2 qAB = 0.3 qAB = 0.4 qAB = 0.5 qAB = 0.6

FIG. 25: Correlation function Cn { Equation (49) } plotted vs. n, for Lb = 64, q = 1.3087, σ = 1, f = 1, N = 12, and various choices of qAB , as indicated. Case (a) refers to a choice of unit vectors from the z-axis to the center of mass of the chain that is grafted at z = i, while case (b) refers to a choice of unit vectors from the z-axis to the center of mass of all monomers of type α in the xy-plane at z = i. Curves are fits to Equation (50).

Brinke [57] introduced a function

P (φ) = ∑

A ′ )δ(|i − j | − φ) (51)

and studied P (φ) varying χAB. However, it turns out that P (φ) always has a rather complicated shape, and its dependence on χAB is rather weak. Thus we investi- gated a related but somewhat different function, namely the histogram P (θ) of the angle θ between the vectors from the axis to the centers of mass of subsequent unlike side chains (Figure 22). We see in this distribution P (θ) also only a rather small dependence on χAB, however: while for qAB = 1 this distribution is essentially struc- tureless for π/2 ≤ θ ≤ 3π/2, for small qAB = 1 a rather pronounced peak at θ ≈ π develops, indicating a prefer- ence of antiparallel orientation of subsequent side chains. However, we feel that such indicators as P (φ) or P (θ) are sensitive only to the presence of short range order rather than long range order, and hence we shall focus on the correlation function Cn in the following. Next we focus on binary bottle brushes in a Theta sol-

vent (q = 1.3087). Figures 23 - 25 show that the results are not very different from the good solvent case: the av- erage number of AB pairs per monomer (not shown) and

the specific heat (Figure 23a) are hardly distinguishable from the good solvent case. Also the radial density pro- file (Figure 23b) exhibits only minor differences, slightly larger densities occur inside the brush than in the good solvent cases, and the transverse component of the end- to-end distance does not exhibit much additional stretch- ing, when qAB decreases (Figure 24a). The distribution P (θ) is somewhat less flat near θ = π (Figure 24b) than in the good solvent case (Figure 22).

Also the correlation function Cn shows again an expo- nential decay with n (Figure 25a), the correlation length ξ being rather similar to the good solvent case (Fig- ure 21). Since one might argue that our definition of a correlation function as given in Equation (49) is not the optimal choice, and there might occur larger corre- lation lengths for a more clever choice of a correlation function, we tried a different choice which is also easy to compute. Namely, in the xy-plane at the index i of the z-coordinate we determine the center of mass of the monomers of type α = A or B in that plane (the choice of α is dictated by the type of chain grafted at z = i).

Then we introduce an unit vector ~Sαi from the z-axis in the direction towards this center of mass. In terms of these unit vectors, which then no longer distinguish from which chain the monomers α in the i’th xy-plane are com- ing, we can again apply the definition, Equation (49) to derive a correlation function. This correlation function is shown in Figure 25b. One sees that the qualitative be- havior of both types of correlation functions is the same, but the decay of this second type of correlation function even is slightly faster than that of the correlation function used previously. Since normally, when one studies prob- lems involving a phase transition, the correlation length of the order parameter is the largest correlation length that one can find in the system, the previous definition (focusing on the location of the center of mass of the in- dividual side chains) seems preferable to us. It is possible of course that such differences between different ways of measuring correlations along the backbone remain so pro- nounced for small N only, where the correlation lengths are only of the order of a few lattice spacings, and hence are less universal and depend on the details of the studied quantity.

We now turn to the poor solvent case (Figures 26 - 29). Already the snapshot picture of the bottle brush poly- mer conformations (Figure 26) reveals that now the side chains adopt much more compact configurations, due to the collapse transition that very long single chains would experience in a poor solvent. [45] If now qAB becomes small, one recognizes a more pronounced phase separa- tion along the backbone of the polymer, although there still is no long range order present.

Still, neither the variation of the average number of AB pairs per monomer mAB/(Nnc) with qAB (Figure 27a) nor the specific heat (Figure 27b) give a hint for the oc- currence of a phase transition: in fact, these data still look like in the good solvent case, Figure 18! Also the distribution P (θ) and the variation of (R2

x+R2 y)/N2/3

20

(a)

(b)

(c)

FIG. 26: Snapshot pictures of bottle brush conformations for Lb = 64, q = 1.5, N = 18, σ = 1, and three choices of qAB , namely qAB = 1.5 (a), qAB = 0.6 (b) and qAB = 0.1 (c). Monomers A, monomers B, and a straight rigid backbone are shown in black, light gray, and white colors, respectively.

with N and qAB are qualitatively similar to the results found for good solvents and Theta solvents, and there- fore are not shown here. More interesting is the monomer density profile (Figure 28). While for N = 6 it still has the same character as in the previous cases, for N = 12 and N = 18 we recognize an inflection point. In fact, for a collapsed polymer bottle brush we expect a profile exhibiting a flat interior region at melt densities (ρ(r) near to ρ = 1), then an interfacial region where ρ(r) rapidly decreases towards zero; in the ideal case reached for q → ∞, the profile should even be a Heaviside step function, in the continuum limit, ρ(r) = θ(h − r). Obvi- ously, for q = 1.5 we are still far from this behavior even for N = 18, but we can identify an interface location at about rint ≈ 3.5, and in the interior of the cylindrical bot- tle brush (for r < rint) the monomer density corresponds at least to a concentrated polymer solution.

Figure 29 then shows again plots of Cn vs. n, and the resulting fits to Equation (50). The behavior is qualita- tively similar to the previous cases of good and Theta solvents again, but now the decay of Cn with n is clearly much slower, indicating a distinctly larger correlation length. This result corroborates the qualitative observa- tion made already on the basis of the snapshot pictures, Figure 26, and quantifies it.

Our findings on the local character of phase separa- tion in binary bottle brush polymers are now summa- rized in Figure 30, where plots of the inverse correlation length 1/ξ versus the inverse Flory-Huggins parameter zc/χ = kBT/(AB − AA) = 1/ ln[q/qAB] are shown (cf. Equation (28) and remember our choice AA = BB). This choice of variables is motivated by the analogy with the XY model in cylindrical geometry, Equation (45); on the basis of this analogy, we would expect that ξ−1 ∝ T ,

i.e. we expect straight lines that extrapolate through zero as T → 0. Figure 30 demonstrates that this analogy [58] clearly

is not perfect. Rather the data are compatible with an extrapolation

ξ−1(N, T ) = ξ−1(N, q, 0) + CN (q)T , T → 0 , (52)

where CN (q) is a coefficient that decreases with increas- ing N and depends on solvent quality and with a nonzero intercept ξ−1(N, q, 0) implying that even in the ground state (T = 0) there is lack of long range order! A very interesting question concerns the dependence

of ξ(N, T ) on chain length. Figure 31 presents a plot of ξ−1(N, q, 0), as estimated from extrapolation of the data shown in Figure 30 to qAB = 0, as a function of 1/N . Indeed the data are compatible with a rela- tion ξ−1(N, q, 0) ∝ 1/N , implying long range order for N → ∞ in the ground state. In principle, carrying out the same extrapolation at nonzero temperature and test- ing for which temperature range ξ−1(N → ∞, T ) starts to be nonzero, one could obtain an estimate for the criti- cal point of intramolecular phase separation, that should occur (and then is well defined) in the limit of infinite side chain length, N → ∞. Unfortunately the accuracy of our estimates for ξ(N, T ) does not warrant such an analysis. The reason for this surprising persistence of disorder

at low temperatures is configurational entropy, of course. As long as q < ∞, the bottle brush polymer is not fully compact, and when the density is small enough inside the bottle brush (as it still is in the cases shown in Fig- ure 28), the two types of chains A, B can avoid mak- ing binary contacts (as is evident from Figures 18 and 27): mAB → 0 as qAB → 0. Hence there is a per-

21

(a)

0

0.03

0.06

0.09

0.12

< m

C v

N = 6

N = 12

N = 18

FIG. 27: (a) Average number of AB pairs per monomers, < mAB > /(Nnc), plotted vs. qAB for side chain lengths N = 6, 12, and 18. All data refer to σ = 1.5, Lb = 64. (b) Specific heat per monomer, Cv/(Nnc), plotted vs. qAB for N = 6, 12, and 18.

0

0.1

0.2

0.3

0.4

0.5

N = 18

N = 12

N = 6

FIG. 28: Radial density profile ρ(r) plotted vs. r for Lb = 64, qAB = 0.1, q = 1.5, σ = 1, f = 1, and three choices of N = 6, 12, and 18.

fect avoidance of energetically unfavorable contacts in the ground state, and the finite correlation length ξ(N, 0) and nonzero entropy of the ground state are not a conse- quence of “frustrated interactions”[107] as in spin glasses, random field spin models, etc. [107, 108]. In the present problem, if both q and N are not too large, a ground state (for q → 0) occurs where the structure of the bottle brush is NOT a cylinder with an interface separating an A-rich and a B-rich domain, as hypothesized in Figure 14!

(a)

0

0.1

0.2

0.3

0.4

n

qAB = 0.1 qAB = 0.2 qAB = 0.3 qAB = 0.4 qAB = 0.5 qAB = 0.6

(b)

0

0.1

0.2

0.3

0.4

0.5

n

qAB = 0.1 qAB = 0.2 qAB = 0.3 qAB = 0.4 qAB = 0.5 qAB = 0.6

(c)

0

0.1

0.2

0.3

0.4

0.5

0.6

C n

n

qAB = 0.1 qAB = 0.2 qAB = 0.3 qAB = 0.4 qAB = 0.5 qAB = 0.6

FIG. 29: Same as Figure 21, but for poor solvent conditions (q = 1.5); for n = 6 (a), n = 12 (b), and n = 18 (c).

Thus a (coarse-grained) cross section of the bottle brush in the xy-plane is NOT a circle, separating A-rich and B-rich regions by a straight line, but rather looks like the number 8, i.e. a dumbbell-like shape, where a (more or less circular and more or less compact A-rich region) oc- curs for x < 0, a similar B-rich region occurs for x > 0, but no monomers (apart from the backbone monomer) occur at the y-axis at x = 0. The orientation of the x-axis can fluctuate as one moves along the z-axis, and unlike Figure 15 (twisting an interface in a cylinder along the z-axis clearly involves an energy cost, and this is de- scribed by the helicity modulus in the XY-model analogy, Equation (45)) the free energy cost of this structural dis- tortion is outweighed by the configurational entropy gain, at least for q and N not too large. It is an unresolved question whether some critical value qc(N) exists, where ξ−1(N, q, 0) vanishes, and a long range ordered ground

22

(a)

0

0.2

0.4

0.6

(b)

0

0.2

0.4

0.6

1/ ξ

zc / χAB

N = 18

N = 12

(c)

0

0.2

0.4

N = 6 Lb = 32 Lb = 48 Lb = 64

FIG. 30: Plot of the inverse correlation length 1/ξ versus the inverse Flory Huggins parameters, zc/χ, for good solvent conditions (q = 1), case (a), Theta solvent conditions (q = 1.3087), case (b), and poor solvent conditions (q = 1.5), case (c). Data for three chain lengths N = 6, 12, and 18 are included throughout. In several cases two or three choices of backbone lengths Lb = 32, 48 and 64 are included as well. All data refer to the choice of one grafted polymer per grafting site (σ = 1).

state occurs. Another unresolved question is, whether (another?) critical value q′c(N) exists, where the charac- ter of the ground state changes such that the local cross section of the binary bottle brush changes from an 8- shaped to a circular density distribution. Actually, the problem of alternatingly grafting A-chains and B-chains along a line is equivalent to grafting symmetric AB di- block copolymers along a line, such that the junction points of the diblocks form a straight line. This prob- lem is the lower-dimensional analog of diblocks grafted with their junction points to the flat interface between

0

0.1

0.2

0.3

0.4

Lb = 32 Lb = 48 Lb = 64

FIG. 31: Inverse correlation length plotted vs. 1/N , in the limit qAB → 0, for poor solvent conditions (q = 1.5), and three choices of the backbone length Lb, to exclude that the data are strongly affected by finite size artifacts. The straight line indicates that the data are compatible with a simple linear relation, ξ−1(N, 0) ∝ 1/N .

an unmixed binary (A,B) homopolymer blend: for this problem it is well-known (see Werner et al. [109] for ref- erences) that the shape of the diblocks is dumbbell like, the A-block being stretched away from the interface, in order to be embedded in the A-rich phase underneath of the interface, and the B-rich block also being stretched away from the interface, in order to be embedded in the B-rich phase above the interface. As a consequence of our discussion, we call into

question the idea of the “Janus cylinder”-type phase separation [56, 57, 58] and propose as an alternative pos- sibility (Figure 32) the “double cylinder” (with cross sec- tion resembling the number 8). Which of these cross- sectional structures occur will depend on the interac- tion parameters AA = BB, and AB, of course. If the strength of the attractive interactions |AA| = |BB| exceeds the strength of the repulsion |AB| sufficiently much, it is clear that for T → 0 the Janus cylinder type phase separation will occur, while in the opposite limit, when |AB| exceeds |AA| = |BB| sufficiently much, the double cylinder geometry will win. In the macroscopic continuum limit a comparison of the respective surface energies would imply that the double cylinder geometry, which avoids an AB interface, but requires for the same volume taken by

Hsiao-Ping Hsu, Wolfgang Paul, and Kurt Binder Institut fur Physik, Johannes Gutenberg-Universitat, D-55099 Mainz, Germany

Summary: Scaling predictions and results from self- consistent field calculations for bottle-brush polymers with a rigid backbone and flexible side chains under good solvent conditions are summarized and their validity and applicability is assessed by a comparison with Monte Carlo simulations of a simple lattice model. It is shown that under typical conditions, as they are also present in experiments, only a rather weak stretching of the side chains is realized, and then the scaling predictions based on the extension of the Daoud-Cotton blob picture are not applicable.

Also two-component bottle brush polymers are consid- ered, where two types (A,B) of side chains are grafted, as- suming that monomers of different kind repel each other. In this case, variable solvent quality is allowed for, such that for poor solvent conditions rather dense cylinder- like structures result. Theories predict “Janus Cylinder”- type phase separation along the backbone in this case. The Monte Carlo simulations, using the pruned-enriched Rosenbluth method (PERM) then are restricted to rather short side chain length. Nevertheless, evidence is ob- tained that the phase separation between an A-rich part of the cylindrical molecule and a B-rich part can only occur locally. The correlation length of this microphase separation can be controlled by the solvent quality. This lack of a phase transition is interpreted by an analogy with models for ferromagnets in one space dimension.

I. Introduction

Flexible macromolecules can be grafted to various sub- strates by special endgroups. Such “polymer brushes” find widespread applications[1, 2, 3, 4, 5] and also pose challenging theoretical problems, such as an understand- ing of the conformational statistics and resulting geomet- rical structure of these tethered chain molecules. Only this latter aspect shall be considered in the present pa- per, for chains grafted to a straight line or a very nar- row cylinder. This problem is a limiting case of “bot- tle brush” polymers where side chains are grafted to a long macromolecule that forms the backbone of the bot- tle brush. When this backbone chain is also a flexible polymer and the grafting density is not very high, a “comb polymer”[6] results, which is outside of consider- ation here. Also we shall not discuss the case where the backbone chain is very short, so the conformation would resemble a “star polymer”.[7, 8, 9, 10, 11] Here we restrict attention to either stiff backbone chains or high graft- ing density of side chains at flexible backbones. In the

lattice case stiffening of the backbone occurs due to ex- cluded volume interactions, and a cylindrical shape of the molecule as a whole results. In fact, many experiments have been carried out where with an appropriate chemical synthesis bottle brush polymers with a worm-like cylin- drical shape were produced [12, 13, 14, 15, 16]. The recent papers[14, 15, 16] contain a more detailed bibliography on this rapidly expanding field. On the theoretical side, two aspects of the confor-

mation of bottle brush polymers where mostly dis- cussed: (i) conformation of a side chain when the back- bone can be treated as a rigid straight line or thin cylinder[10, 17, 18, 19, 20, 21, 22, 23, 24, 25, 26, 27] (ii) confor- mation of the whole bottle brush when the backbone is (semi)flexible.[28, 29, 30, 31, 32, 33, 34, 35, 36, 37, 38, 39, 40]

The latter problem is left out of consideration in the present paper. Problem (i), the stretching of the side chains in the radial direction in the case of sufficiently high grafting density, was mostly discussed in terms of a scaling description, [10, 17, 18, 19, 20, 24, 25, 26] extending the Daoud-Cotton [8] “blob picture”[41, 42, 43] from star polymers to bottle brush polymers. If one uses the Flory exponent[44, 45] ν = 3/5 in the scaling relation for the average root mean square end-to-end distance of a side chain, Re ∝ σ(1−ν)/(1+ν)N2ν/(1+ν), where σ is the graft- ing density and N is the number of effective monomeric units of a side chain, one obtains Re ∝ σ1/4N3/4. These exponents happen to be identical to those which one would obtain assuming that the chains attain quasi- two-dimensional configurations, resulting if each chain is confined to a disk of width σ−1.[27] Although this lat- ter picture is a misconception, in experimental studies (e.g. [14, 15]) this hypothesis of quasi-two-dimensional chains is discussed as a serious possibility. Therefore we find it clearly necessary to first review the correct scaling theory based on the blob picture, and discuss in detail what quantities need to be recorded in order to distin- guish between these concepts. Thus, in the next section we shall give a detailed discussion of the scaling concepts for bottle brush polymers with rigid backbones. Thereafter we shall describe the Monte Carlo test

of these predictions, that we have recently per- formed using the pruned enriched Rosenbluth method (PERM).[46, 47, 48, 49] After a brief description of the Monte Carlo methodology, we present our numerical re- sults and compare them to the pertinent theoretical pre- dictions. In the second part of this paper, we discuss the

extension from one-component to two-component bot- tle brush polymers. Just as in a binary polymer blend (A,B) typically the energetically unfavorable in-

teraction (described by the Flory-Huggins parameter χ [44, 45, 50, 51, 52]) should cause phase separation be- tween A-rich and B-rich domains. However, just as in block copolymers where A chains and B-chains are tethered together in a point,[53, 54, 55] no macroscopic phase separation but only “microphase separation” is possible: for a binary (A,B) bottle brush with a rigid backbone one may expect formation of “Janus Cylin- der” structures.[56, 57, 58] This means, phase separation occurs such that the A-chains assemble in one half of the cylinder, the B chains in the other half, separated from the A-chains via a flat interface containing the cylinder axis. However, it has been argued that the long range order implied by such a “Janus cylinder” type struc- ture has a one-dimensional character, and therefore true long range order is destroyed by fluctuations at nonzero temperature.[58] Only local phase separation over a finite correlation length along the cylinder axis may persist.[58]

We shall again first review the theoretical background on this problem, and then describe the simulation evi- dence. We conclude our paper by a summary and out- look on questions that are still open, briefly discussing also possible consequences on experimental work. How- ever, we shall not deal with the related problems of mi- crophase separation of a bottle brush with only one kind of side chains induced by deterioration of the solvent quality[59, 60] or by adsorption on flat substrates.[61, 62, 63]

II. Conformation of Side Chains of Bottle Brushes under Good Solvent Conditions: Theoretical Background

The most straightforward approach to understand the conformations of chains in polymer brushes and star polymers under good solvent conditions uses the con- cept to partition the space available for the chains into compartments, called “blobs”. The idea is that in each such region there occur only monomers of one chain, no monomers of any other chains occur in such a blob, and hence self-avoiding walk statistics holds in each blob. This means, if a (spherical) blob has a radius rB and contains n monomers, these numbers must be related via

rB = anν , ν ≈ 0.588 , n 1 . (1)

Here a is a length of the order of the size of an effec- tive monomer, and we emphasize from the start that it is crucial to use the correct value of the self-avoiding walk exponent ν, as it is provided from renormalization group calculations[64] or accurate Monte Carlo simulations.[65]

If one would ignore the small difference between ν and the Flory estimate 3/5, one would already miss an impor- tant distinction between two different scaling regimes for a brush on a flat substrate.[66] An almost trivial condi- tion of this “blobology”[43] is that each of the N effective monomeric units of a chain must belong to some blob.

So we have

N = nnB , (2)

where nB is the number of blobs belonging to one par- ticular chain. Finally we note that the space available to the chains

must be densely filled with blobs. It then remains to discuss which factors control the blob size rB.

[43] The simplest case is a polymer brush on a flat substrate (un- der good solvent conditions, as assumed here through- out): if we neglect, for simplicity, any local fluctuations in the grafting density, the distance between grafting sites simply is given by σ−1/2. Putting rB = σ−1/2 in Equation (1), we find n = (σa2)−1/2ν , i.e. each chain is a string of nB = N/n = N(σa2)1/2ν blobs. Accord- ing to the simple-minded description of polymer brushes due to Alexander,[41] this string simply is arranged like a one-dimensional cigar, and one would conclude that the height of a flat brush is

h = σ−1/2nB = Na(σa2)1/(2ν)−1/2 . (3)

The free end of the chain is in the last blob and hence the end-to-end distance Re ≈ h in this “Alexander picture” of polymer brushes.[1, 41, 42, 43] However, a more detailed theory of polymer brushes, such as the self-consistent field theory in the strong stretching limit,[67, 68, 69] yields a somewhat different behavior: the end monomer is not localized at the outer edge of the brush, but rather can be located anywhere in the brush, according to a broad dis- tribution; also the monomer density in polymer brushes at flat substrates is not constant up to the brush height h, but rather decreases according to a parabolic profile. So even for a polymer brush at a flat substrate already a description in terms of non-uniform blob sizes, that increase with increasing distance z from the substrate, is required.[70] However, in the following we shall disre- gard all these caveats about the Alexander picture for flat brushes, and consider its generalization to the bottle brush geometry, where polymer chains are tethered to a line rather than a flat surface. Then we have to partition space into blobs of nonuniform size and shape in order to respect the cylindrical geometry (Figure 1). In the discussion of brushes in cylindrical geometry in

terms of blobs in the literature[19, 20, 26] the non-spherical character of the blob shape is not explicitly accounted for, and it rather is argued that one can characterize the blobs by one effective radius ξ(r) depending on the radial dis- tance r from the cylinder axis. One considers a segment of the array of length L containing p polymer chains.[19]

On a surface of a cylinder of radius r and length L there should then be p blobs, each of cross-sectional area ξ2(r); geometrical factors of order unity are ignored throughout. Since the surface area of the cylindrical segment is Lr, we must have[19, 20, 26]

pξ2(r) = Lr , ξ(r) = (Lr/p)1/2 = (r/σ)1/2 . (4)

If the actual non-spherical shape of the blobs (Figure 1) is neglected, the blob volume clearly is of the order of

3

r

(b)

FIG. 1: Schematic construction of a blob picture for star polymer (a), and for a bottle brush (b), (c). We assume that along the rigid backbone there occur at a regular spacing fσ−1 grafting sites where at each grafting site f side chains containing N effective monomeric units are grafted. If the rigid backbone of the cylindrical bottle brush is oriented along the z-axis, part (c) shows a view of the blob partitioning in the xy-plane perpendicular to the backbone, while part (b) shows a cut through the cylinder along the xz-plane containing the cylinder axis. A few possible chain configurations are indicated. While for a star polymer the blobs have a spherical shape, their radius ξ(r) increasing linearly proportional to the distance r from the center of the star (a), for the bottle brush the blobs are ellipsoids with three axes ξ(r) (in x-direction), proportional to r/f (in y-direction), and fσ−1 (in z-direction), respectively. For a considered chain the x-axis contains the center of mass of the chain.

ξ3(r) = (r/σ)3/2. Invoking again the principle that in- side a blob self-avoiding walk statistics hold, we have, in analogy with Equation (1),

ξ(r) = a[n(r)]ν , n(r) = [ξ(r)/a]1/ν = [r/(σa2)]1/2ν . (5)

From this result one immediately derives the power law decay for the density profile ρ(r) as follows[3, 19, 20, 26]

ρ(r) = n(r)/ξ3(r) = a−3[r/(σa2)]−(3ν−1)/2ν

≈ a−3[r/(σa2)]−0.65 (6)

Using the Flory approximation[44, 45] ν = 3/5 one would find ρ(r) ∝ r−2/3 instead.

Now the average height h of the bottle brush is esti- mated by requiring that we obtain all σN monomers per unit length in the z-direction along the axis of the bottle brush (cf. Figure 1) when we integrate ρ(r) from r = 0 to r = h,

σN =

h∫

0

N = (σa)(ν−1)/(2ν)(h/a)(ν+1)/(2ν), (8a)

4

h/a = (σa)(1−ν)/(1+ν)N2ν/(1+ν) = (σa)0.259N0.74 . (8b)

Note that the use of the Flory estimate ν = 3/5 would simply yield h ∝ σ1/4N3/4, which happens to be identical to the relation that one obtains when one partitions the cylinder of height L and radius h into disks of height σ−1, requiring hence that each chain is confined strictly into one such disk. Then each chain would form a quasi-two- dimensional self-avoiding walk formed from n′

blob = N/n′

blobs of diameter σ−1. Since we have σ−1 = an′ν again, we would conclude that the end-to-end distance R of such a quasi-two-dimensional chain is

R = σ−1(n′

blob) 3/4 = σ−1n′−3/4N3/4

= a(σa)−1+3/4νN3/4 = a(σa)1/4N3/4 . (9)

Putting then R = h, Equation (8b) results when we use there ν = 3/5. However, this similarity between Equa- tions (8b), (9) is a coincidence: in fact, the assump- tion of a quasi-two-dimensional conformation does not imply a stretching of the chain in radial direction. In fact, when we put the x-axis of our coordinate system

in the direction of the end-to-end vector ~R of the chain, we would predict that the y-component of the gyration radius scales as

Rgy = a(σa)1/4N3/4 , (10)

since for quasi-two-dimensional chains we have Rgx ∝ Rgy ∝ R, all these linear dimensions scale with the same power laws. On the other hand, if the Daoud-Cotton- like[8] picture {Figure 1a} holds, in a strict sense, one would conclude that Rgy is of the same order as the size of the last blob for r = h,

Rgy = ξ(r = h) = (h/σ)1/2

= a(σa)−ν/(1+ν)Nν/(1+ν) (11)

Clearly this prediction is very different from Equa- tion (10), even with the Flory exponent ν = 3/5 we find from Equation (11) that Rgy ∝ σ−3/8N3/8. Hence it is clear that an analysis of all three components of the gy- ration radius of a polymer chain in a bottle brush is very suitable to distinguish between the different versions of scaling concepts discussed in the literature. However, at this point we return to the geometrical

construction of the filling of a cylinder with blobs, Fig- ure 1. We explore the consequences of the obvious fact that the blobs cannot be simple spheres, when we re- quire that each blob contains monomers from a single chain only, and the available volume is densely packed with blobs touching each other. As mentioned above, ξ(r) was defined from the avail-

able surface area of a cylinder at radius r, cf. Equa- tion (4). It was argued that for each chain in the surface area Lr of such a cylinder a surface area ξ2(r) is available. However, consideration of Figure 1 shows that these sur- faces are not circles but rather ellipses, with axes fσ−1

and r/f . The blobs hence are not spheres but rather

ellipsoids, with three different axes: fσ−1 in z-direction along the cylinder axes, r/f in the y-direction tangential on the cylinder surface, normal to both the z-direction and the radial direction, and the geometric mean of these two lengths (rσ−1)1/2, in the radial x-direction. Since the physical meaning of a blob is that of a volume region in which the excluded volume interaction is not screened, this result implies that the screening of excluded volume in a bottle brush happens in a very anisotropic way: there are three different screening lengths, fσ−1 in the axial z- direction, (rσ−1)1/2 in the radial x-direction, and r/f in the third, tangential, y-direction. Of course, it remains to be shown by a more microscopic theory that such an anisotropic screening actually occurs. However, the volume of the ellipsoid with these three

axes still is given by the formula

Vellipsoid = (σ−1f)(r/f)(rσ−1)1/2 = (rσ−1)3/2 = [ξ(r)]3

(12) with ξ(r) given by Equation (4), and hence the volume of the blob has been correctly estimated by the spherical approximation. As a consequence, the estimations of the density profile ρ(r), Equation (6), and resulting brush height h, Equation (8b), remain unchanged. More care is required when we now estimate the linear

dimensions of the chain in the bottle brush. We now ori- ent the x-axis such that the xz-plane contains the center of mass of the considered chain. As Figure 1b indicates, we can estimate Rgz assuming a random walk picture in terms of blobs. When we go along the chain from the grafting site towards the outer boundary of the bottle brush, the blobs can make excursions with z = ±fσ−1, independent of r. Hence we conclude, assuming that the excursions of the nblob steps add up randomly

R2 gz =

Rgz = fσ−1√nblob . (13)

Hence we must estimate the number of blobs nblob per chain in a bottle brush. We must have

nblob =

[ξ(r)]−1dr (14)

Note from Figure 1 that we add an increment 2ξ(ri) to r when we go from the shell i to shell i+ 1 in the cylin- drical bottle brush. So the discretization of the integral in Equation (14) is equivalent to the sum. From Equa- tion (14) we then find, again ignoring factors of order unity

nblob = σ1/2h1/2 = (σa)1/(1+ν)Nν/(1+ν) , (15)

and consequently

5

With Flory exponents we hence conclude nblob ∝ σ5/8N3/8, and thus Rgz ∝ fσ−11/16N3/16. The estima- tion of Rgy is most delicate, of course, because when we consider random excursions away from the radial direc- tions, the excursions y = ±ξ(r) are non-uniform. So we have instead of Equation (13),

R2 gy =

σ−1/2h3/2 and hence

∝ σ−0.055N0.555 (18)

while the corresponding result with Flory exponents is Rgy ∝ σ−1/16N9/16. These different results for Rgx ∝ h {Equation (8b)}, Rgy {Equation (18)} and Rgz {Equation (16)} clearly reflect the anisotropic struc- ture of a chain in a bottle brush. Note that the result for Rgy according to Equation (18) is much larger than the simple Daoud-Cotton-like prediction, Equation (11), but is clearly smaller than the result of the quasi-two- dimensional picture, Equation (10). As a consistency check of our treatment, we note that

also Equation (7) can be formulated as a discrete sum over blobs

N =

[r/(σa)]1/2ν−1/2dr ,

(19) which yields Equation (8a), as it should be. Finally we discuss the crossover towards mushroom be-

havior. Physically, this must occur when the distance between grafting points along the axis, fσ−1, becomes equal to aNν . Thus we can write

h = aNνh(σaNν), (20)

where we have absorbed the extra factor f in the scaling function h(ζ). We note that Equation (8b) results from Equation (20) when we request that

h(ζ 1) ∝ ζ(1−ν)/(1+ν), (21)

and hence a smooth crossover between mushroom be- havior and radially stretched polymer conformations oc- curs for σaNν of order unity, as it should be. Analogous crossover relations can be written for the other linear di- mensions, too:

Rgz = aNνRgz(ζ), Rgz(ζ 1) ∝ ζ−(2ν+1)/(2ν+2), (22)

Rgy = aNνRgy(ζ), Rgy(ζ 1) ∝ ζ−(2ν−1)/(2ν+2), (23)

The agreement between Equation (16) and Equation (22) or Equation (18) and Equation (23), respectively, pro- vides a check on the self-consistency of our scaling argu- ments.

However, it is important to bear in mind that the blob picture of polymer brushes, as developed by Alexander,[41] Daoud and Cotton,[8] Halperin[1, 43] and many others, is a severe simplification of reality, since its basic assumptions that (i) all chains in a polymer brush are stretched in the same way, and (ii) the chain ends are all at a distance h from the grafting sites, are not true. Treatments based on the self-consistent field theory[67, 68, 69, 71, 72, 73, 74, 75, 76] and computer simulations[3, 22, 66, 70, 77, 78, 79, 80, 81, 82, 83] have shown that chain ends are not confined at the outer bound- ary of the brush, and the monomer density distribution is a nontrivial function, that cannot be described by the blob model. However, it is widely believed that the blob model yields correctly the power laws of chain linear di- mensions in terms of grafting density and chain length, so the shortcomings mentioned above affect the pre-factors in these power laws only. In this spirit, we have extended the blob model for brushes in cylindrical geometry in the present section, taking the anisotropy in the shape of the blobs into account to predict the scaling behavior of both the brush height h (which corresponds to the chain end-to-end distance R and the x-component Rgx of the gyration radius) and of the transverse gyration ra- dius components Rgy , Rgz. To our knowledge, the latter have not been considered in the previous literature.

III. Monte Carlo Methodology

We consider here the simplest lattice model of poly- mers under good solvent conditions, namely, the self- avoiding walk on the simple cubic lattice. The backbone of the bottle brush is just taken to be the z-axis of the lattice, and in order to avoid any effects due to the ends of the backbone, we choose periodic boundary conditions in the z-direction. The length of the backbone is taken to be Lb lattice spacings, and the lattice spacing henceforth is taken as one unit of length. Note that in order to avoid finite size effects Lb has to be chosen large enough so that no side chain can interact with its own “images” created by the periodic boundary condition, i.e. Rgz Lb.

We create configurations of the bottle brush poly- mers applying the pruned-enriched-Rosenbluth method (PERM).[46, 47, 48, 49, 87, 88, 89, 90] This algorithm is based on the biased chain growth algorithm of Rosen- bluth and Rosenbluth,[91] and extends it by re-sampling technique (“population control”[46]) with depth-first implementation. Similar to a recent study of star polymers[47, 48] all side chains of the bottle brush are grown simultaneously, adding one monomer to each side chain one after the other before the growth process of the first chain continues by the next step.

6

FIG. 2: Snapshot picture of a bottle brush polymer with Lb = 128 σ = 1/4, and N = 2000 on the simple cubic lattice. Note that different chains are displayed in different colors to distinguish them, and the periodic boundary condition is un- done for the sake of a better visibility in the visualization of this configuration.

When a monomer is added to a chain of length n− 1 (containing n monomers) at the nth step, one scans the neighborhood of the chain end to identify the free neigh- boring sites of the chain end, to which a monomer could be added. Out of these nfree sites available for the addi- tion of a monomer one site is chosen with the probability pn,i for the ith direction. One has the freedom to sam- ple these steps from a wide range of possible distribu- tions, e.g. pn,i = 1/nfree, if one site is chosen at random, and this additional bias is taken into account by suitable weight factors. The total weight Wn of a chain of length n with an unbiased sampling is determined recursively by Wn = Πnk=1wk = Wn−1wn. While the weight wn is gained at the nth step with a probability pn,i, one has to use wn/pn,i instead of wn. The partition sum of a chain of length n (at the nth step) is approximated as

Zn ≈ Zn ≡M−1 n

Mn∑ α=1

Wn(α), (24)

where Mn is the total number of configurations {α}, and averages of any chain property (e.g. its end-to-end dis- tance, gyration radius components, etc.) A(α) are ob- tained as

An = 1

Zn (25)

As is well-known from Ref. [84], for this original biased sampling[91] the statistical errors for large n are very hard to control. This problem is alleviated by popula- tion control.[87] One introduces two thresholds

W+ n = C+Zn, W−

n = C−Zn , (26)

where Zn is the current estimate of the partition sum, and C+ and C− are constants of order unity. The opti- mal ratio between C+ and C− is found to be C+/C− ∼ 10 in general. If Wn exceeds W+

n for the configuration α, one produces k identical copies of this configuration, re- places their weight Wn by Wn/k, and uses these copies as members of the population for the next step, where one adds a monomer to go from chain length n to n+ 1. However, if Wn < W−

n , one draws a random number η, uniformly distributed between zero and one. If η < 1/2, the configuration is eliminated from the population when one grows the chains from length n to n+1. This “prun- ing” or “enriching” step has given the PERM algorithm its name. On the other hand, if η ≥ 1/2, one keeps the configuration and replaces its weight Wn by 2Wn. In a depth-first implementation, at each time one deals with only a single configuration until a chain has been grown either to the end of reaching the maximum length or to be killed in between, and handles the copies by recursion. Since only a single configuration has to be remembered during the run, it requires much less memory.

In our implementation, we usedW+ n = ∞ andW−

n = 0 for the first configuration hitting chain length n. For the following configurations, we usedW+

n = CZn(cn/c0) and W− n = 0.15W+

n , here C = 3.0 is a positive constant, and cn is the total number of configurations of length n al- ready created during the run. The bias of growing side chains was used by giving higher probabilities in the di- rection where there are more free next neighbor sites and in the outward directions perpendicular to the backbone, where the second part of bias decreases with the length of side chains and increases with the grafting density. To- tally 105 ∼ 106 independent configurations were obtained in most cases we simulated.

Typical simulations used backbone lengths Lb = 32, 64, and 128, f = 1 (one chain per grafting site of the backbone, although occasionally also f = 2 and f = 4 were used), and grafting densities σ = 1/32, 1/16, 1/8, 1/4, 1/2 and 1. The side chain length N was varied up to N = 2000. So a typical bottle brush with Lb = 128, σ = 1/4 (i.e., nc = 32 side chains) and N = 2000 contains a total number of monomers Ntot = Lb + ncN = 64128. Figure 2 shows a snapshot configuration of such a bottle brush polymer. Note that most other simulation algo- rithms for polymers[65, 84, 85, 86] would fail to produce a large sample of well-equilibrated configurations of bottle brush polymers of this size: dynamic Monte Carlo al- gorithms using local moves involve a relaxation time (in units of Monte Carlo steps per monomer [MCS]) of or- der Nz where z = 2ν + 1 if one assumes that the side chains relax independently of each other and one ap- plies the Rouse model[92] in the good solvent regime.[85]

For N = 2000 such an estimate would imply that the time between subsequent statistically independent con- figurations is of the order of 107 MCS, which clearly is impractical. While the pivot algorithm[65] would pro- vide a significantly faster relaxation in the mushroom regime, the acceptance rate of the pivot moves quickly

7

deteriorates when the monomer density increases. This algorithm could equilibrate the outer region of the bottle brush rather efficiently, but would fail to equilibrate the chain configurations near the backbone. The configura- tional bias algorithm[86, 93] would be an interesting alter- native when the monomer density is high, but it is not expected to work for very long chains, such as N = 2000. Also, while the simple enrichment technique is useful to study both star polymers[94] and polymer brushes on flat substrates[95] it also works only for chain lengths up to about N = 100. Thus, existing Monte Carlo simulations of one-component bottle brushes under good solvent con- ditions either used the bond fluctuation model[85, 96] on the simple cubic lattice applying local moves with side chain lengths up to N = 41[30] or N = 64[36] or the pivot algorithm[65] with side chain lengths up to N = 80,[34]

but considering flexible backbone of length L = 800. An alternative approach was followed by Yethiraj[31] who studied an off-lattice tangent hard sphere model by a pivot algorithm in the continuum, for N ≤ 50. All these studies addressed the question of the overall conforma- tion of the bottle brush for a flexible backbone, and did not address in detail the conformations of the side chains. Only the total mean square radius of gyration of the side chains was estimated occasionally, obtaining[30, 36]

R2 g ∝ N1.2 or[31] R2

g ∝ N1.36 and[34] R2 g ∝ N1.4. How-

ever, due to the smallness of the side chain lengths used in these studies, as quoted above, these results have to be considered as somewhat preliminary, and also a sys- tematic study of the dependence on both N and σ was not presented. We also note that the conclusions of the quoted papers are somewhat contradictory. An interesting alternative simulation method to the

Monte Carlo study of polymeric systems is Molecular Dynamics,[85] of course. While in corresponding stud- ies of a bead-spring model of polymer chains for flat brushes[81] chain lengths N up to N = 200 were used, for chains grafted to thin cylinders[22] the three chain lengths N = 50, 100 and 150 were used. For N = 50, also four values of grafting density were studied.[22] Mu- rat and Grest[22] used these data to test the scaling pre- diction for the density profile, Equation (6), but found that ρ(r) is better compatible with ρ(r) ∝ r−0.5 rather than ρ(r) ∝ r−0.65. However, forN = 50 the range where the power law is supposed to apply is very restricted, and hence this discrepancy was not considered to be a prob- lem for the theory.[22]

Thus, we conclude that only due to the use of the PERM algorithm has it become possible to study such large bottle brush polymers as depicted in Figure 2. Nev- ertheless, as we shall see in the next section, even for such large side chain lengths one cannot yet reach the asymp- totic region where the power laws derived in the previous section are strictly valid.

IV. Monte Carlo Results for One- Component Bottle-Brush Polymers

(a)

2

1.5

1

< R

x2 > /

N

σ = 1/4 σ = 1/8 σ = 1/16 σ = 1/32 σ = 1/64 σ = 1/128

(b)

0.1

0.095

0.09

0.085

< R

y2 > /

N

σ = 1/4 σ = 1/8 σ = 1/16 σ = 1/32 σ = 1/64 σ = 1/128

(c)

0.6

0.5

0.4

0.3

< R

z2 > /

N

σ = 1/128 σ = 1/64 σ = 1/32 σ = 1/16 σ = 1/8 σ = 1/4

FIG. 3: Log-log plot of the mean square end-to-end distance components R2

x (a), R2

y (b), and R2

z (c) versus side chain length N , for various choices of the grafting density σ as indi- cated. All data refer to f = 1 (one chain per possible grafting site) and N > 5. Note that the x-direction for every chain is the normal direction from its center of mass position to the bottle brush backbone. All data are for Lb = 128. The chain mean square linear dimensions are all normalized by N2ν .

In Figures 3 and 4, we present our data for the mean square end-to-end radii and gyration radii components of the side chains. Note that for each chain configuration a separate local coordinate system for the analysis of the chain configuration needs to be used; while the z-axis is always oriented simply along the backbone, the x-axis is oriented perpendicular to the z-axis and goes through the center of mass of the chain in this particular config- uration. The y-axis then also is fixed simply from the requirement that it is perpendicular to both the x- and z-axes.

For a polymer mushroom (which is obtained if the

8

(a)

0.3

0.2

0.1

< R

/ N

2ν

N

σ = 1/4 σ = 1/8 σ = 1/16 σ = 1/32 σ = 1/64 σ = 1/128

(b)

0.04

0.038

< R

/ N

2ν

N

σ = 1/4 σ = 1/8 σ = 1/16 σ = 1/32 σ = 1/64 σ = 1/128

(c) 0.13

< R

/ N

2ν

N

σ = 1/128 σ = 1/64 σ = 1/32 σ = 1/16 σ = 1/8 σ = 1/4

FIG. 4: Log-log plot of the mean square gyration radius com- ponents R2

gx (a), R2

gy (b), and R2

gz (c), versus side chain length N . Only data for N > 10 are included. All data are for f = 1, Lb = 128, and various choices of σ. All chain mean square linear dimensions are normalized by N2ν with ν = ν3 ≈ 0.588.

grafting density σ is sufficiently small) we expect that all chain linear dimensions scale as Nν , for sufficiently long chains. Therefore we have normalized all mean square linear dimensions in Figures 3 and 4 by a factor N2ν , using the theoretical value[64, 65] ν = 0.588. However, as we see from Figures 3, 4 in the range 10 ≤ N ≤ 103 dis- played there, even for the smallest σ presented, where a single side chain is simulated, the shown ratios are not constant. This fact indicates that corrections to scaling[64, 65] should not be disregarded, and this prob- lem clearly complicates the test of the scaling predic- tions derived above. For the largest value of σ included (σ = 1/4), the irregular behavior of some of the data (Figure 3b,c, Figure 4b) indicate a deterioration of sta-

(a) 2.2

(R 2 x+

R 2 y)

(R 2 x+

R 2 y)

⊥ = R2

y divided by N2ν

vs. ζ = σNν , including all data for N > 5, and three choices of Lb as indicated (a), or alternatively removing data affected by the finite size of the backbone length via the periodic bound- ary condition (b). The slope indicated in (b) by the dotted straight line corresponds to the scaling estimate from Equa- tion (21), 2(1− ν)/(1 + ν) ≈ 0.519.

tistical accuracy. This problem gets worse for increasing number of side chains nc.

A further complication is due to the residual finite size effect. Figure 5 shows a plot of R2

⊥ = R2

x + R2 y vs. the

scaling variable ζ = σNν . One can recognize that for small Lb but large N and not too large σ systematic deviations from scaling occur (Figure 5a), which simply arise from the fact that an additional scaling variable (related to R2

z1/2/Lb) comes into play when R2 z1/2 no

longer is negligibly smaller than Lb. While for real bot- tle brush polymers with stiff backbone effects due to the finite lengths of the backbone are physically meaningful and hence of interest, the situation is different in our simulation due to the use of periodic boundary condi- tions. The choice of periodic boundary conditions is mo- tivated by the desire to study the characteristic structure in a bottle brush polymer far away from the backbone ends, not affected by any finite size effects. However, if R2

gz1/2 becomes comparable to Lb, each chain interacts with its own periodic images, and this is an unphysical, undesirable, finite size effect. Therefore in Figure 5b, the data affected by such finite size effects are not included. One finds a reasonable data collapse of the scaled mean square end-to-end distance when one plots the data ver- sus the scaling variable ζ = σNν . These results consti-

9

(a)

0.5

0.1

< R

gx2 > /

N 2ν

ζ = σNν

slope = 0.519

σ = 1/128 σ = 1/64 σ = 1/32 σ = 1/16 σ = 1/8 σ = 1/4

(b)

0.5

0.1

< R

gy2 > /

N 2ν

ζ = σNν

slope = -0.111

σ = 1/128 σ = 1/64 σ = 1/32 σ = 1/16 σ = 1/8 σ = 1/4

(c)

0.5

0.1

< R

gz2 > /

N 2ν

ζ = σNν

slope = -1.370

σ = 1/128 σ = 1/64 σ = 1/32 σ = 1/16 σ = 1/8 σ = 1/4

FIG. 6: Log-log plot of R2

gx/N2ν (a), R2

gy/N2ν (b) and R2

gz/N2ν (c) versus the scaling variable ζ = σNν , using the data in Figure 4 but for N > 50. The slopes indicated by dashed straight lines illustrate the scaling estimates from Equation (21), 2(1 − ν)/(1 + ν) ≈ 0.519 (a), from Equa- tion (23), −(2ν − 1)/(ν + 1) ≈ −0.111 (b), and from Equa- tion (22), −(2ν + 1))/(ν + 1) ≈ −1.370 (c).

tute the first comprehensive test of the scaling relations for bottle brush polymers, Equations (21) - (23), and the consistency between the data and the proposed scaling structure in terms of the variable ζ is indeed very grati- fying. On the other hand, it is also evident from Figures 5 and 6 that only a mild stretching of the side chains away from the backbone is observed, and in this region one is still far away from the region of strong stretching, where the simple power laws Equations (8b), (18) and (16) ap- ply. Obviously, the crossover from the simple mushroom behavior (observed for ζ = σNν 1) to the strongly stretched bottle brush (observed for ζ 1) takes at least one decade of the scaling variable ζ. There is a rather

(a)

0.001

0.01

0.1

< R

N

σ = 1 σ = 1/3 σ = 1/7 σ = 1/15 σ = 1/31 σ = 1/63

(b)

0.001

0.01

0.1

< R

N

σ = 1 σ = 1/3 σ = 1/7 σ = 1/15 σ = 1/31 σ = 1/63

(c)

0.01

0.1

1

10

100

1000

< R

σ = 1/63 σ = 1/31 σ = 1/15 σ = 1/7 σ = 1/3

FIG. 7: Log-log plot of the mean-square gyration radius com- ponents R2

gx,slit/N2ν2 (a), R2

gy,slit/N2ν2 (b) and R2

gz,slit (c) versus side chain length N with ν2 = 3/4. As in Fig- ure 4, only data for N > 5 are included. Various choices of σ are included. Note that the walls of the slit are located at z = ±(σ−1 + 1)/2 and are strictly repulsive hard walls. One chain end is fixed at the x-axis at z = 0, and since the x-axis represents the backbone if this polymer in a slit is taken as a model of a disk-shaped section of a bottle brush, all sites of the x-axis are excluded from occupation of the monomers of the (side) chain as well.

gradual and smooth crossover rather than a kink-like be- havior of the scaling function. While in the x-component at least near ζ = 10 a weak onset of stretching can be recognized, hardly any evidence for the contraction of the y and z-components is seen.

In order to test what one would expect if the picture of the chains as quasi-two-dimensional self-avoiding walks were correct, we have also studied single chains grafted to a straight backbone of length σ, σ = 1, 1/3, 1/5, . . .1/63

10

(a)

0.01

0.1

1

< R

(b)

0.01

0.1

1

< R

(c)

1e-05

1e-04

0.001

0.01

0.1

1

< R

FIG. 8: Log-log plot of Rgx,slit/N2ν (a), R2

gy,slit/N2ν , and

R2

gzslit/N2ν (c) versus the scaling variable ζ = σNν . Only data for N > 10 are included. The slopes indicated by dashed straight lines illustrate the scaling exponent implied by Equa- tion (27), namely 3/2ν − 2 (a,b) and −2 (c), respectively. In (c) σ−1 is replaced by σ−1 + 1 to remove a finite-size effect.

which are confined between two parallel repulsive infinite walls. The grafting site of the chains was chosen at the site located symmetrically between the confining walls in the slit {if the grafting site is chosen to be the origin of the coordinate system, the confining hard walls occur at z = ±(σ−1 + 1)/2}. Figure 7 gives log-log plots of the gyration radii components of such chains confined to such disk-like slits, which we denote as Rgα, slit, α = x, y and z, in order to distinguish then from the actual gyration radii components of the side chains in a bottle brush polymer. One can clearly see that R2

gx,slit, R2 gy,slit

scale as N2ν2 = N3/2 for large N , as it must be. These data are very similar to data for chains confined between

(a)

1

σ = 1/63 σ = 1/31 σ = 1/15 σ = 1/7 σ = 1/3

(b)

0.1

1

σ = 1/63 σ = 1/31 σ = 1/15 σ = 1/7 σ = 1/3

(c)

1

10

100

1000

σ = 1/3 σ = 1/7 σ = 1/15 σ = 1/31 σ = 1/63

FIG. 9: Log-log plot of R2

gx/R2

gz/R2

gz,slit versus N , for values of σ strictly cor- responding to each other, as indicated.

repulsive walls without a grafting to a piece of a rigid backbone,[97] of course. In the corresponding scaling plot (Figure 8) one can see that both R2

gx,slit and R 2 gy,slit have

the simple crossover scaling behavior[45, 98]

R2 gx,slit = N2ν fx(σN

ν) (27)

with fx(ζ) ∝ fy(ζ) ∝ ζ2(ν2−ν)/ν with ν2 = 3/4, as ex-

pected, and seen in related previous work.[97, 99] Obvi- ously, although we use in Figures 7 and 8 the same range of N and σ as in Figures 4 and 6, the behavior is rather different. As expected from our scaling analysis pre- sented above, the confinement that a chain experiences in a bottle brush due to the presence of the other chains is much weaker than the confinement of a chain in the equivalent disk-like sector between confining walls. This

11

(a)

1e-04

0.001

0.01

0.1

1

slope = -0.65

σ = 1/128 σ = 1/64 σ = 1/32 σ = 1/16 σ = 1/8 σ = 1/4

(b)

1e-04

0.001

0.01

0.1

1

slope = -0.65

σ = 1/128 σ = 1/64 σ = 1/32 σ = 1/16 σ = 1/8 σ = 1/4

(c)

1e-04

0.001

0.01

0.1

1

slope = -0.65

σ = 1/128 σ = 1/64 σ = 1/32 σ = 1/16 σ = 1/8 σ = 1/4

FIG. 10: Radial distribution function ρ(r) plotted vs. r, for N = 500 (a), N = 1000 (b), and N = 1500 (c), for various choices of σ, as indicated. Note that due to the discreteness of the lattice, the number N(r) of monomers in the interval [r, r+dr] is not normalized by the factor πr that applies in the continuum limit, but by the number Nr of lattice sites (x,y) satisfying the constraint r2 = x2 + y2, i.e.

P

r N(r) = N and

ρ(r) = N(r)/Nr . All data refer to Lb = 128 and f = 1.

fact is demonstrated very directly in Figure 9, where the ratios R2

gα/R2 gα,slit are plotted vs. N for the corre-

sponding values of σ. If the hypothesis of quasi-two di- mensional confinement were valid, we would expect these ratios to be constants. Obviously, this is not the case.

As a final point of this section, we discuss the distri- bution of monomers (Figures 10 and 11) and chain ends (Figures 12 and 13) in the simulated model for the bottle brush polymer. Unlike corresponding radial density dis- tributions for the off-lattice bead-spring model of Murat and Grest,[22] where for small distances close to the back- bone a kind of “layering” was observed, we see a rather

(a)

0

5

10

15

20

< ρ(

z) >

z

σ = 1/128 σ = 1/64 σ = 1/32 σ = 1/16 σ = 1/8

(b)

0

5

10

15

20

25

< ρ(

z) >

z

σ = 1/128 σ = 1/64 σ = 1/32 σ = 1/16 σ = 1/8

(c)

0

5

10

15

20

25

30

< ρ(

z) >

z

σ = 1/128 σ = 1/64 σ = 1/32 σ = 1/16 σ = 1/8

FIG. 11: Density distribution function ρ(z) plotted vs. the coordinate z along the backbones, for N = 500 (a), N = 1000 (b), and N = 1500 (c), and various choices of σ, as indicated. This distribution is normalized by choosing

P

z ρ(z) = 1

smooth behavior also for small distances (Figure 10). For larger distances, the behavior is qualitatively very sim- ilar. Again we fail to provide a clear-cut evidence for the predicted power law decay, Equation (6). Note, how- ever, that this power law is supposed to hold only in the strong stretching limit, where Equation (8b) is ob- servable (which we do not verify either), and in addition the stringent condition 1 r h needs to be obeyed, to have this power law. Although our simulations en- compass much longer chains than every previous work on bottle brushes, we clearly fail to satisfy this double inequality. Turning to the distribution along the backbone (Fig-

ure 11), the periodicity due to the strictly periodic spac- ing of grafting sites is clearly visible. If desired, one could also study a random distribution of grafting sites along

12

(a)

0

2

4

6

8

< ρ e

σ = 1/128 σ = 1/64 σ = 1/32 σ = 1/16 σ = 1/8

(b)

4

6

8

10

12

< ρ e

σ = 1/128 σ = 1/64 σ = 1/32 σ = 1/16 σ = 1/8

(c)

10

12

14

< ρ e

σ = 1/128 σ = 1/64 σ = 1/32 σ = 1/16 σ = 1/8

FIG. 12: Density distributions of chain ends ρe(z) plotted vs. z, for the same choice of parameters as in Figure 11.

the backbone, of course, but we have restricted attention to the simplest case of a regular arrangement of grafting sites only. The distribution of chain ends ρ(z) exhibits an analogous periodicity for small values of σ only, while ρe(z) is approximately constant (Figure 12) for larger values of σ.

Most interesting is the radial distribution of chain ends (Figure 13). One can see an increasing depression of ρe(r) for small r when σ increases. Again these data are similar to the off-lattice results of Murat and Grest.[22] In no case do we see the “dead zone” predicted by the self-consistent field theory in the strong stretching limit,[21, 24] however.

V. Phase Separation in Two-Component Bottle Brushes: Theoretical Background

(a)

0

0.02

0.04

0.06

0.08

0.1

< ρ e

nd (r

r

σ = 1/128 σ = 1/64 σ = 1/32 σ = 1/16 σ = 1/8 σ = 1/4

(b)

0

0.02

0.04

0.06

0.08

0.1

< ρ e

nd (r

r

σ = 1/128 σ = 1/64 σ = 1/32 σ = 1/16 σ = 1/8 σ = 1/4

(c)

0

0.02

0.04

0.06

0.08

0.1

< ρ e

nd (r

r

σ = 1/128 σ = 1/64 σ = 1/32 σ = 1/16 σ = 1/8 σ = 1/4

FIG. 13: Radial density distribution of chain ends ρe(r) plot- ted vs. r, for the same choice of parameters as in Figures 10- 12.

We still consider a bottle brush polymer with a strictly rigid straight backbone, where at regularly distributed grafting sites (grafting density σ) side chains of length N are attached, but now we assume that there are two chemically different monomeric species, A and B, com- posing these side chains with NA = NB = N . These systems have found recent attention, suggesting the pos- sibility of intramolecular phase separation. [56, 57, 58] In a binary system pairwise interaction energies AA, AB, and BB are expected, and consequently phase separation between A and B could be driven by the Flory-Huggins parameter

χ = zc/kBT, = AB − (AA + BB)/2 (28)

where zc is the coordination number of the lattice, like in the Flory-Huggins lattice model of phase separation in

13

y

FIG. 14: Schematic description of perfect phase separation of side chains in a cylindrical binary (A,B) bottle brush poly- mer into a “Janus cylinder” structure, where the A-chains occupy the lower hemicylinder and the B-chains occupy the upper hemicylinder. The interface between B-rich and A-rich phases is assumed to be oriented in the yz-plane. The figure indicates the characterization of this order in terms of a local order parameter, namely the vector ~ψ(z) oriented normal to the interface at every grafting site. The absolute value of this vector characterizes a suitable average of the local phase sep- aration in a disk of the cylinder located at z (see text). For

perfect order | ~ψ(z) | = 1 and ~ψ(z) is oriented along the same axis for the whole bottle brush polymer.

a binary polymer blend. [44, 45, 50, 51, 52] However, since the side chains are grafted to the backbone, only in- tramolecular phase separation is possible here. Actu- ally, the energy parameter suffices for dense polymer blends or dense block copolymer melts, where no solvent is present. [44, 45, 50, 51, 52] For the problem of intramolec- ular phase separation in a bottle brush, the solvent can- not be disregarded and hence the enthalpy of mixing rather is written as.[52, 56]

Emix/kBT =

∫ dV

+ χABφA(~r)φB(~r)], (29)

where v is the volume per monomer, φA(~r), φB(~r) and φS(~r) are the local volume fractions of monomers of types A and B, and the solvent density, respectively, and three pairwise interaction parameters χAS , χBS, and χAB en- ter. The latter χAB corresponds to the χ-parameter writ- ten in Equation (28), while the former two control the solvent quality for polymers A and B, respectively. Of course, using the incompressibility condition

φA(~r) + φB(~r) + φS(~r) = 1 (30)

the solvent density can be eliminated from the problem (but one should keep in mind that in the free energy density there is an entropy of mixing term φS(~r) lnφS(~r) present [56]). In the framework of the lattice model stud- ied here, v ≡ 1 and solvent molecules are only implicitly considered, identifying them with vacant sites. For sim- plicity, the following discussion considers only the most symmetric case, where χAS = χBS , and the numbers of A chains and B chains are equal. Stepanyan et al. [56] used Equations (29) and (30),

as the starting point of a self-consistent field calcula-

tion, adding conformational free energy contributions ac- counting for the entropy associated with the stretching of Gaussian chains. It is found that when χAB exceeds a critical value χ∗

AB, intramolecular phase separation of “Janus cylinder”-type occurs (Figure 14). Then an in- terface is formed, containing the backbone of the bottle brush, such that there is an excess of A-monomers below the interface and an excess of B-monomers above the in- terface (or vice versa). Assuming that at the position z of the backbone the interface is oriented in x-direction, we can describe this Janus-type phase separation in terms of an one-dimensional order parameter density

ψ(z) = (n+ B−n+

B are the numbers of A(B) monomers

in the interval [z, z + dz] with x > 0(n+ A, n

+ B) and x <

A, n −

B), respectively. Since we shall see below that the orientation of the interface is an important degree of freedom, we may consider ψ(z) as the absolute value of

a vector order parameter ~ψ(z), and the direction of ~ψ(z) is defined such that ψ(z) takes a maximum. However, Stepanyan et al. [56] did not consider the possibility of an inhomogeneity along the z-axis, and they also did not derive how the order parameter depends on the parame- ters N , σ, and the various χ parameters of the problem {Equation (29)}. Stepanyan et al.[56] also assume that the distribution of chain ends is a delta function at the radius (or “height” h) respectively) of the bottle brush, where h is given by h/a = (σa)1/4N3/4 in the good sol- vent regime. They then find that phase separation occurs for

χ∗

AB ∝ 1/ √ N, (32)

but argue that this result holds only for a “marginal sol- vent” rather than a good solvent, due to the mean-field approximation used which neglects that inside a blob all binary contacts are avoided, estimating the number of contacts simply proportional to the product φAφB , cf. Equation (29), and neglecting the correlations due to excluded volume. The regime of marginal solvents is reached near the θ-point (which occurs for 1 − 2χAS = 1− 2χBS = 0), and requires that [56]

0 < 1− 2χAS < N−1/3 (33)

where again prefactors of order unity are omitted. Stepanyan et al. [56] extend Equation (32) by a simple

scaling-type argument, stating that the transition from the mixed state to the separated state occurs when the energy of the A-B contacts per side chain, E, is of the order of kBT . They estimate this energy as

E/kBT ≈ Np(φ)χAB , (34)

where p(φ) is the probability of the A-B contact, which depends on the average volume fraction φ of the monomers inside the brush. According to the mean field

14

A

A

B

B

y

FIG. 15: Same as Figure 14, but allowing for a long wave-

length variation of the vector ~ψ(z) characterizing the local interface orientation in the Janus cylinder.

cT

ξ

R

T

0

FIG. 16: Schematic sketch of the temperature dependence of the correlation length ξ of the ferromagnetic XY-model in a cylinder of radius R.

theory, p(φ) ∝ φ, where φ = N/h2, h being the ra- dius of the cylindrical brush. Using h ∝ N3/4 (Equa- tion (8b)) one finds p(φ) ∝ N−1/2 and using this result in Equation (34) implies E/kBT ∝ N1/2χAB, and from E/kBT = 1 we recover Equation (32). The merit of this simple argument is that it is readily

extended to other cases: e.g., for a θ-solvent, we have[18]

h ∝ N2/3 and hence p(φ) ∝ N−1/3, yielding [56]

χ∗

AB ∝ N−2/3 , θ − solvent. (35)

For the poor solvent case, the bottle brush should col- lapse to a cylinder densely filled with monomers, and hence h ∝ N1/2, φ = 1, and thus

χ∗

AB ∝ N−1 , poor solvent. (36)

Note that Equation (36) is the same relation as for a dense bulk polymer blend or block copolymer melt, respectively.[44, 45, 50, 51, 52]

The situation is more subtle in the good solvent case, however, since there the probability of contact is no longer given by the mean field result p(φ) ∝ φ but rather by [45]

p(φ) ∝ φ5/4 ∝ N−5/8 , (37)

where the Flory approximation ν = 3/5 was again used, with φ ∝ N−1/2 when h ∝ N3/4. Equations (34) and

(37) now imply

AB ∝ N−3/8 , good solvent (38)

However, these crude estimates do not suffice to prove that for χAB > χ∗

AB true long range order of this “Janus

cylinder” type (Figure 14) is established. Hsu et al.[58]

suggested that there is also the need to consider varia-

tions of the direction of the order parameter ~ψ(z) along the z-direction (Figure 15). It was argued that for any finite side chain length N also the cylinder radius (or brush “height”) h is finite, and hence the system is one-dimensional. In one-dimensional systems with short range interactions at nonzero temperatures no long range order is possible.[100, 101] The situation depicted in Fig- ure 15 is reminiscent of the one-dimensional XY-model of a chain of spins on a one-dimensional lattice where each spin at site i is described by an angle i in the xy- plane, with 0 ≤ i ≤ 2π, and where neighboring spins are coupled. This coupling is described by the Hamiltonian

H = −J ∑ i

~Si+1 · ~Si (39)

when ~Si = (cosi, sini) is a unit vector in the xy-plane. While mean field theory predicts that ferromagnetic or- der occurs along the chain, for ferromagnetic exchange J > 0 and temperatures T less than the critical tem- perature TMF

c which is of the order of J/kB, the exact solution of this model, Equation (39), shows[100, 101] that Tc = 0, since ferromagnetic long range order is unstable against long wavelength fluctuations. One can show that the spin-spin correlation function for large z = a(j − i) decays to zero exponentially fast,

~Si · ~Sj ∝ exp[−z/ξ], z → ∞ (40)

where a is the lattice spacing of this spin chain. The correlation length ξ gradually grows as the temperature is lowered,

ξ = 2a(J/kBT ) (41)

Equation (41) is at variance with mean field theory, which rather would predict[100] (the index MF stands for “mean field” throughout)

ξMF ∝ (T/TMF c − 1)−νMF , νMF = 1/2 . (42)

This critical divergence at a nonzero critical tempera- ture TMF

c is completely washed out by the fluctuations: rather than diverging at TMF

c , the actual correlation length ξ {Equation (41)} at TMF

c still is only of the order of the lattice spacing. This consideration can be generalized to spin sys-

tems on lattices which have a large but finite size in (d − 1) dimensions and are infinite in one space dimen- sions only.[102, 103] E.g., when we consider an infinitely

15

long cylinder of cross section πR2 we expect that Equa- tions (41), (42) are replaced by the finite size scaling relation [104, 105]

ξ = ξ∞ ξ(R/ξ∞) , ξ(ζ 1) = 1 , ξ(ζ 1) ∝ ζ , (43)

where ξ∞ is the correlation length of the XY model on a lattice which is infinitely large in all d = 3 directions of space.

ξ∞ ∝ (T/Tc − 1)−ν , (44)

where again kBTc ∝ J (but with a smaller constant of proportionality than that in the relation kBT

MF c ∝ J),

and ν is the correlation length exponent of the XY model (ν ≈ 0.67).[106] Equation (43) describes a smooth crossover of the ferromagnetic correlation length describ- ing spin correlations along the axis of the cylinder from bulk, Equation (44), to a quasi-one-dimensional varia- tion. For T Tc the correlation length resembles Equa- tion (41), since[102, 103]

ξ = 2πΓ(T )R2/kBT ≈ 2π(R2/a)(J/kBT ), T → 0. (45)

the “helicity modulus” (also called “spin wave stiffness”) Γ(T ) is of order J for T → 0 and shows a critical vanish- ing as T → Tc from below, in the thermodynamic limit R → ∞. However, for finite R there is a finite size round- ing of this singularity of Γ(T → Tc), such that Γ(T = Tc) is of order 1/R, and hence a smooth crossover to Equa- tion (43) occurs near Tc. Figure 16 gives a qualitative account of this behavior. For more details of this finite size crossover we refer to the literature.[102, 103] But we suggest a qualitatively similar behavior for the domain size ξ of segregated A-rich and B-rich domains in binary bottle brush polymers. So, when we study the correla- tion function of the order parameter considered in Equa- tion (31)

Gψ(z) = ~ψ(z′) · ~ψ(z′ + z) ∝ exp(−z/ξψ) (46)

we expect that the correlation length ξψ describing the lo- cal phase separation in the direction along the backbone of the bottle brush polymer remains of order unity as long as χ−1

AB exceeds χ∗ −1 AB distinctly. For χAB near χ∗

AB we expect that ξψ becomes of order h, the radius of the bottle brush. For χAB χ∗

AB, we expect ξψ ∝ h2χAB, by analogy with Equation (45). Unfortunately, the test of those predictions even in the poor solvent case where χ∗ −1 AB is largest, is rather difficult, since the prefactor in

the relation χ∗ AB ∝ 1/N is unknown.

VI. Monte Carlo Results for Binary Bottle Brush Polymers

We use the same lattice model as considered before in our Monte Carlo study of the chain conformations of

one-component bottle brush polymers, but now in the construction of the weights Wn(α) we have to take into account that the partition function now is

Z = ∑ α

qmAA+mBBqmAB

AB (47)

with (remember that we restrict attention to the choice AA = BB)

q = exp(−AA/kBT ), qAB = exp(−AB/kBT ) . (48)

In Equation (47) the numbers of non-bonded occupied nearest-neighbor monomer pairs AA, BB and AB are de- noted as mAA,mBB and mAB, respectively. Note that the sum in Equation (47) extends over all possible con- figurations {α} of the bottle brush polymer. The choice q = qAB = 1 corresponds to the previously studied one- component bottle brush under good solvent conditions, while the choice q = qAB > 1 corresponds to variable solvent quality for the one-component brush (note that q = qAB means χ = 0, Equation (28), and also χAB which is proportional to χ then vanishes: this means there is no chemical incompatibility between A and B any longer, no physical difference between A and B ex- ists any more). From previous work on single chains[46]

we know that the θ-point occurs for qθ = 1.3087. There- fore we varied q in the range 1 ≤ q ≤ 1.5; q = 1.5 hence falls in the regime of poor solvent quality already. Of course, in order to have rather compact configurations of cylindrical bottle brushes a choice of much larger q would be desirable. However, the efficiency of the PERM algo- rithm quickly deteriorates with increasing q: for q = 1.5 we encounter already for rather small values of the side chain length N such as N = 18 and a backbone length of Lb = 64 huge statistical fluctuations. The total size of the bottle brush polymer under poor solvent condi- tions reached here, Ntot = NσLb + Lb = 1216, is al- most two orders of magnitude smaller than the maxi- mal size studied under good solvent conditions! How- ever, all known simulation algorithms for polymers suffer from difficulties of equilibration in the limit of very dense configurations. [84, 85, 86]

Since we are mostly interested in the high grafting limit (σ = 1, so the number of side chains nc = σLb = Lb) in the PERM algorithm where all side chains grow simultaneously we use a bias factor such that side chains are grown with higher probability in the direc- tions perpendicular to the backbone. This additional bias (which is not present in the standard Rosenbluth [91]

and PERM[46] methods) must be taken into account by suitable weight factors. About 106 independent configu- rations were typically generated. Figures 17 - 19 now show typical results for the good

solvent case (q = 1) but varying the parameter qAB con- trolling the chemical incompatibility. The visual inspec- tion of the configurations (Figure 17) reveals little in- fluence of qAB, however, and this observation is corrob- orated by the more quantitative analysis: the average

16

(a)

(b)

(c)

FIG. 17: Snapshot pictures of bottle brush configurations for Lb = 64, q = 1, N = 18, σ = 1 and three choices of qAB , qAB = 1.0 (a), qAB = 0.4 (b) and qAB = 0.1 (c). Monomers A, monomers B, and a straight rigid backbone are shown in black, light gray, and white colors, respectively.

(a)

0

0.03

0.06

0.09

0.12

0.15

< m

C v

N = 6

N = 12

N = 18

FIG. 18: (a) Average number of AB pairs per monomer mAB/(Nnc) plotted vs. qAB for side chain lengths N = 6, 12, and 18. All data refer to σ = 1, Lb = 64. (b) Specific heat per monomer, cv/(Nnc) plotted vs. qAB for N = 6, 12 and 18.

(a)

0

0.1

0.2

0.3

0.4

(< R

x2 > +

< R

y2 > )

qAB=0.1

qAB=0.5

qAB=1.0

FIG. 19: (a) Radial density distribution ρ(r) plotted vs. r for Lb = 64, N = 18, q = 1, σ = 1, f = 1 and various qAB . (b) Normalized transverse mean square end-to-end distance (R2

x + R2

y)/N2ν plotted vs. N , for Lb = 64, q = 1, σ = 1, f = 1, and three choices of qAB as shown.

17

x

y

3

n

FIG. 20: Vectors ~Rα cm(n) from the grafting site n to the xy-

component of the center of mass of the respective chain, and corresponding unit vectors (denoted by arrows). For a per- fectly phase separated structure with the interface between A and B being the yz plane, for α = A all unit vectors point along the negative x-axis and for α = B all unit vectors point along the positive x-axis.

(a)

0

0.1

0.2

n

qAB = 0.1 qAB = 0.2 qAB = 0.3 qAB = 0.4 qAB = 0.5 qAB = 0.6

(b)

0

0.1

0.2

0.3

n

qAB = 0.1 qAB = 0.2 qAB = 0.3 qAB = 0.4 qAB = 0.5 qAB = 0.6

(c)

0

0.1

0.2

0.3

C n

n

qAB = 0.1 qAB = 0.2 qAB = 0.3 qAB = 0.4 qAB = 0.5 qAB = 0.6

FIG. 21: Correlation function Cn measuring local “Janus cylinder”-type phase separation plotted versus n, for N = 6 (a), 12 (b), and 18 (c). Various choices of qAB are included, as indicated in the figure. Curves show fits to Equation (50). All data refer to good solvent conditions (q = 1), and Lb = 64, σ = 1, f = 1.

(a)

0

0.05

0.1

0.15

0.2

0.25

0.3

P (θ

θ / π

qAB = 0.1 qAB = 0.2 qAB = 0.4 qAB = 0.6 qAB = 0.8 qAB = 1.0

(b)

0

0.05

0.1

0.15

0.2

0.25

0.3

P (θ

θ / π

qAB = 0.1 qAB = 0.2 qAB = 0.4 qAB = 0.6 qAB = 0.8 qAB = 1.0

FIG. 22: Distribution P (θ) of the angle θ between the vectors towards the centers of mass of subsequent (unlike) side chains plotted vs. θ/π, for N = 12 (a) and N = 18 (b). Various choices of qAB are included, as indicated.

number of A-B pairs per monomer is extremely small (Figure 18a) even for qAB = 1, and hence not much enthalpy could be won if A-chains and B-chains avoid each other: due to the excluded volume interaction, very few nearest neighbor contacts between any non-bonded monomers occur in our bottle brush model. For N = 18 and qAB = 1 the total number of AB contacts per chain is only about 1.4, and increases with increasing N only very slowly. So for the range of side chain lengths ac- cessible in our work, no phase separation should be ex- pected. In the specific heat one does see a weak peak near 0.2 ≤ qAB ≤ 0.4, but the height of this peak decreases very strongly with increasing N . Furthermore does nei- ther the peak position shift with increasing N (as one would expect from Equation (38), if this peak would be a rounded precursor of the phase transition that should occur at χ∗

AB in the limit N → ∞) nor does the peak width decrease with increasing N . Thus, it is clear that this peak is not an indicator of a “Janus-cylinder”-type phase separation in the bottle brush: rather we interpret it as a Schottky-type anomaly, expected from the fact that in our model of alternatingly grafted A-and B-chains at a straight line backbone with coordinates (0, 0, z) in the immediate environment of the backbone (e.g. at lat- tice sites (x, y, z) = (±1, 0, z) or (0,±1, z)) there is a nonzero a-priori probability of 1/4 that between the first monomer of the chain grafted at z and the first monomer of the chain grafted at z + 1 a nearest-neighbor contact

18

(a)

0

0.01

0.02

0.03

0.04

C v

(b)

0

0.1

0.2

0.3

0.4

qAB = 0.1

qAB = 0.3

qAB = 0.5

FIG. 23: (a) Specific heat per monomer, CN/(Nnc), plotted vs. qAB for N = 6, 12, and 18 for σ = 1, Lb = 64, and q = 1.3087 (a Theta solvent). (b) Radial density distribution ρ(r) plotted vs. r for Lb = 64, N = 18, q = 1.3087, σ = 1, f = 1, and three choices of qAB .

occurs. The finite energy from this local contacts near the backbone gives rise to the peak in the specific heat. Also the radial density profile (Figure 19a) shows lit-

tle effects of varying qAB , and there is also no effect in the gyration radius component R2

g⊥ = R2 gx + R2

gy of the side chains, although a weak increase occurs in the corresponding component of the end-to-end distance (Figure 19b). In the latter figure, one can see for small N an even-odd oscillation, but this lattice effect clearly has died out for N > 10. In order to test for correlations measuring local phase

separation along the backbone, Equation (46) is some- what cumbersome to implement numerically, since for

each z one has to find the direction of ~ψ(z) from the

condition that |~ψ(z)| is maximal (cf. Equation (31)). A simpler and similar correlation function has been defined from the vectors pointing from the grafting site i to the center of mass of the respective side chains. Projecting this vector into the xy-plane and defining an unit vector ~Sαi (α = A or B) along this projection (Figure 20) we define a correlation function Cn as follows

Cn ≡ [~SAi · ~SAi+n+ ~SBi+1 · ~SBi+1+n]/2 . (49)

Here we have explicitly incorporated the alternating grafting ABAB... of side chains along the backbone. The average . . . in Equation (49) includes an averaging over

(a)

1

1.2

1.4

1.6

(< R

x2 > +

< R

y2 > /

N

N

P (θ

FIG. 24: (a) Normalized transverse mean square end-to-end distance (< R2

x > + < R2

y >)/N plotted vs. N , for Lb = 64, σ = 1, f = 1, and q = 1.3087 (Theta solvent). Three choices of qAB are included. (b) Distribution P (θ) of the angle be- tween the vectors towards the centers of mass of subsequent (unlike) side chains plotted vs. θ/π, for N = 18, other param- eters as in (a).

all sites {i} on which A chains are grafted, in order to im- prove the statistics. If perfect long range order occurs, as implied in Figure 20, we clearly have Cn = 1 independent of n, while for the case of short range order, we expect Cn ∝ exp(−n/ξ). Actually, considering the fact that we use a periodic boundary condition, we have analyzed our numerical data in terms of the ansatz

Cn ∝ {exp(−n/ξ) + exp[−(Lb − n)/ξ]} . (50)

Figure 21 shows our data for Cn for the three choices of N : indeed we recognize that Cn decays to zero with in- creasing n, but the increase does get slower with increas- ing side chain length N . The scale of this correlation effect clearly increases with decreasing qAB. While for N = 6 the correlation length ξ hardly depends on qAB, for large N a slight increase of ξ with decreasing qAB is suggested.

In an earlier simulation study of phase separation in binary bottle brushes, [57] it was suggested to quantify the degree of separation by considering the distribution of the polar angle i from the axis to monomer . Defining a variable σA , which is σA = 1 if monomer is of type A and zero otherwise, and similarly σB , de Jong and ten

19

(a)

0

0.1

0.2

0.3

0.4

n

qAB = 0.1 qAB = 0.2 qAB = 0.3 qAB = 0.4 qAB = 0.5 qAB = 0.6

(b)

0

0.1

0.2

0.3

0.4

0.5

n

qAB = 0.1 qAB = 0.2 qAB = 0.3 qAB = 0.4 qAB = 0.5 qAB = 0.6

FIG. 25: Correlation function Cn { Equation (49) } plotted vs. n, for Lb = 64, q = 1.3087, σ = 1, f = 1, N = 12, and various choices of qAB , as indicated. Case (a) refers to a choice of unit vectors from the z-axis to the center of mass of the chain that is grafted at z = i, while case (b) refers to a choice of unit vectors from the z-axis to the center of mass of all monomers of type α in the xy-plane at z = i. Curves are fits to Equation (50).

Brinke [57] introduced a function

P (φ) = ∑

A ′ )δ(|i − j | − φ) (51)

and studied P (φ) varying χAB. However, it turns out that P (φ) always has a rather complicated shape, and its dependence on χAB is rather weak. Thus we investi- gated a related but somewhat different function, namely the histogram P (θ) of the angle θ between the vectors from the axis to the centers of mass of subsequent unlike side chains (Figure 22). We see in this distribution P (θ) also only a rather small dependence on χAB, however: while for qAB = 1 this distribution is essentially struc- tureless for π/2 ≤ θ ≤ 3π/2, for small qAB = 1 a rather pronounced peak at θ ≈ π develops, indicating a prefer- ence of antiparallel orientation of subsequent side chains. However, we feel that such indicators as P (φ) or P (θ) are sensitive only to the presence of short range order rather than long range order, and hence we shall focus on the correlation function Cn in the following. Next we focus on binary bottle brushes in a Theta sol-

vent (q = 1.3087). Figures 23 - 25 show that the results are not very different from the good solvent case: the av- erage number of AB pairs per monomer (not shown) and

the specific heat (Figure 23a) are hardly distinguishable from the good solvent case. Also the radial density pro- file (Figure 23b) exhibits only minor differences, slightly larger densities occur inside the brush than in the good solvent cases, and the transverse component of the end- to-end distance does not exhibit much additional stretch- ing, when qAB decreases (Figure 24a). The distribution P (θ) is somewhat less flat near θ = π (Figure 24b) than in the good solvent case (Figure 22).

Also the correlation function Cn shows again an expo- nential decay with n (Figure 25a), the correlation length ξ being rather similar to the good solvent case (Fig- ure 21). Since one might argue that our definition of a correlation function as given in Equation (49) is not the optimal choice, and there might occur larger corre- lation lengths for a more clever choice of a correlation function, we tried a different choice which is also easy to compute. Namely, in the xy-plane at the index i of the z-coordinate we determine the center of mass of the monomers of type α = A or B in that plane (the choice of α is dictated by the type of chain grafted at z = i).

Then we introduce an unit vector ~Sαi from the z-axis in the direction towards this center of mass. In terms of these unit vectors, which then no longer distinguish from which chain the monomers α in the i’th xy-plane are com- ing, we can again apply the definition, Equation (49) to derive a correlation function. This correlation function is shown in Figure 25b. One sees that the qualitative be- havior of both types of correlation functions is the same, but the decay of this second type of correlation function even is slightly faster than that of the correlation function used previously. Since normally, when one studies prob- lems involving a phase transition, the correlation length of the order parameter is the largest correlation length that one can find in the system, the previous definition (focusing on the location of the center of mass of the in- dividual side chains) seems preferable to us. It is possible of course that such differences between different ways of measuring correlations along the backbone remain so pro- nounced for small N only, where the correlation lengths are only of the order of a few lattice spacings, and hence are less universal and depend on the details of the studied quantity.

We now turn to the poor solvent case (Figures 26 - 29). Already the snapshot picture of the bottle brush poly- mer conformations (Figure 26) reveals that now the side chains adopt much more compact configurations, due to the collapse transition that very long single chains would experience in a poor solvent. [45] If now qAB becomes small, one recognizes a more pronounced phase separa- tion along the backbone of the polymer, although there still is no long range order present.

Still, neither the variation of the average number of AB pairs per monomer mAB/(Nnc) with qAB (Figure 27a) nor the specific heat (Figure 27b) give a hint for the oc- currence of a phase transition: in fact, these data still look like in the good solvent case, Figure 18! Also the distribution P (θ) and the variation of (R2

x+R2 y)/N2/3

20

(a)

(b)

(c)

FIG. 26: Snapshot pictures of bottle brush conformations for Lb = 64, q = 1.5, N = 18, σ = 1, and three choices of qAB , namely qAB = 1.5 (a), qAB = 0.6 (b) and qAB = 0.1 (c). Monomers A, monomers B, and a straight rigid backbone are shown in black, light gray, and white colors, respectively.

with N and qAB are qualitatively similar to the results found for good solvents and Theta solvents, and there- fore are not shown here. More interesting is the monomer density profile (Figure 28). While for N = 6 it still has the same character as in the previous cases, for N = 12 and N = 18 we recognize an inflection point. In fact, for a collapsed polymer bottle brush we expect a profile exhibiting a flat interior region at melt densities (ρ(r) near to ρ = 1), then an interfacial region where ρ(r) rapidly decreases towards zero; in the ideal case reached for q → ∞, the profile should even be a Heaviside step function, in the continuum limit, ρ(r) = θ(h − r). Obvi- ously, for q = 1.5 we are still far from this behavior even for N = 18, but we can identify an interface location at about rint ≈ 3.5, and in the interior of the cylindrical bot- tle brush (for r < rint) the monomer density corresponds at least to a concentrated polymer solution.

Figure 29 then shows again plots of Cn vs. n, and the resulting fits to Equation (50). The behavior is qualita- tively similar to the previous cases of good and Theta solvents again, but now the decay of Cn with n is clearly much slower, indicating a distinctly larger correlation length. This result corroborates the qualitative observa- tion made already on the basis of the snapshot pictures, Figure 26, and quantifies it.

Our findings on the local character of phase separa- tion in binary bottle brush polymers are now summa- rized in Figure 30, where plots of the inverse correlation length 1/ξ versus the inverse Flory-Huggins parameter zc/χ = kBT/(AB − AA) = 1/ ln[q/qAB] are shown (cf. Equation (28) and remember our choice AA = BB). This choice of variables is motivated by the analogy with the XY model in cylindrical geometry, Equation (45); on the basis of this analogy, we would expect that ξ−1 ∝ T ,

i.e. we expect straight lines that extrapolate through zero as T → 0. Figure 30 demonstrates that this analogy [58] clearly

is not perfect. Rather the data are compatible with an extrapolation

ξ−1(N, T ) = ξ−1(N, q, 0) + CN (q)T , T → 0 , (52)

where CN (q) is a coefficient that decreases with increas- ing N and depends on solvent quality and with a nonzero intercept ξ−1(N, q, 0) implying that even in the ground state (T = 0) there is lack of long range order! A very interesting question concerns the dependence

of ξ(N, T ) on chain length. Figure 31 presents a plot of ξ−1(N, q, 0), as estimated from extrapolation of the data shown in Figure 30 to qAB = 0, as a function of 1/N . Indeed the data are compatible with a rela- tion ξ−1(N, q, 0) ∝ 1/N , implying long range order for N → ∞ in the ground state. In principle, carrying out the same extrapolation at nonzero temperature and test- ing for which temperature range ξ−1(N → ∞, T ) starts to be nonzero, one could obtain an estimate for the criti- cal point of intramolecular phase separation, that should occur (and then is well defined) in the limit of infinite side chain length, N → ∞. Unfortunately the accuracy of our estimates for ξ(N, T ) does not warrant such an analysis. The reason for this surprising persistence of disorder

at low temperatures is configurational entropy, of course. As long as q < ∞, the bottle brush polymer is not fully compact, and when the density is small enough inside the bottle brush (as it still is in the cases shown in Fig- ure 28), the two types of chains A, B can avoid mak- ing binary contacts (as is evident from Figures 18 and 27): mAB → 0 as qAB → 0. Hence there is a per-

21

(a)

0

0.03

0.06

0.09

0.12

< m

C v

N = 6

N = 12

N = 18

FIG. 27: (a) Average number of AB pairs per monomers, < mAB > /(Nnc), plotted vs. qAB for side chain lengths N = 6, 12, and 18. All data refer to σ = 1.5, Lb = 64. (b) Specific heat per monomer, Cv/(Nnc), plotted vs. qAB for N = 6, 12, and 18.

0

0.1

0.2

0.3

0.4

0.5

N = 18

N = 12

N = 6

FIG. 28: Radial density profile ρ(r) plotted vs. r for Lb = 64, qAB = 0.1, q = 1.5, σ = 1, f = 1, and three choices of N = 6, 12, and 18.

fect avoidance of energetically unfavorable contacts in the ground state, and the finite correlation length ξ(N, 0) and nonzero entropy of the ground state are not a conse- quence of “frustrated interactions”[107] as in spin glasses, random field spin models, etc. [107, 108]. In the present problem, if both q and N are not too large, a ground state (for q → 0) occurs where the structure of the bottle brush is NOT a cylinder with an interface separating an A-rich and a B-rich domain, as hypothesized in Figure 14!

(a)

0

0.1

0.2

0.3

0.4

n

qAB = 0.1 qAB = 0.2 qAB = 0.3 qAB = 0.4 qAB = 0.5 qAB = 0.6

(b)

0

0.1

0.2

0.3

0.4

0.5

n

qAB = 0.1 qAB = 0.2 qAB = 0.3 qAB = 0.4 qAB = 0.5 qAB = 0.6

(c)

0

0.1

0.2

0.3

0.4

0.5

0.6

C n

n

qAB = 0.1 qAB = 0.2 qAB = 0.3 qAB = 0.4 qAB = 0.5 qAB = 0.6

FIG. 29: Same as Figure 21, but for poor solvent conditions (q = 1.5); for n = 6 (a), n = 12 (b), and n = 18 (c).

Thus a (coarse-grained) cross section of the bottle brush in the xy-plane is NOT a circle, separating A-rich and B-rich regions by a straight line, but rather looks like the number 8, i.e. a dumbbell-like shape, where a (more or less circular and more or less compact A-rich region) oc- curs for x < 0, a similar B-rich region occurs for x > 0, but no monomers (apart from the backbone monomer) occur at the y-axis at x = 0. The orientation of the x-axis can fluctuate as one moves along the z-axis, and unlike Figure 15 (twisting an interface in a cylinder along the z-axis clearly involves an energy cost, and this is de- scribed by the helicity modulus in the XY-model analogy, Equation (45)) the free energy cost of this structural dis- tortion is outweighed by the configurational entropy gain, at least for q and N not too large. It is an unresolved question whether some critical value qc(N) exists, where ξ−1(N, q, 0) vanishes, and a long range ordered ground

22

(a)

0

0.2

0.4

0.6

(b)

0

0.2

0.4

0.6

1/ ξ

zc / χAB

N = 18

N = 12

(c)

0

0.2

0.4

N = 6 Lb = 32 Lb = 48 Lb = 64

FIG. 30: Plot of the inverse correlation length 1/ξ versus the inverse Flory Huggins parameters, zc/χ, for good solvent conditions (q = 1), case (a), Theta solvent conditions (q = 1.3087), case (b), and poor solvent conditions (q = 1.5), case (c). Data for three chain lengths N = 6, 12, and 18 are included throughout. In several cases two or three choices of backbone lengths Lb = 32, 48 and 64 are included as well. All data refer to the choice of one grafted polymer per grafting site (σ = 1).

state occurs. Another unresolved question is, whether (another?) critical value q′c(N) exists, where the charac- ter of the ground state changes such that the local cross section of the binary bottle brush changes from an 8- shaped to a circular density distribution. Actually, the problem of alternatingly grafting A-chains and B-chains along a line is equivalent to grafting symmetric AB di- block copolymers along a line, such that the junction points of the diblocks form a straight line. This prob- lem is the lower-dimensional analog of diblocks grafted with their junction points to the flat interface between

0

0.1

0.2

0.3

0.4

Lb = 32 Lb = 48 Lb = 64

FIG. 31: Inverse correlation length plotted vs. 1/N , in the limit qAB → 0, for poor solvent conditions (q = 1.5), and three choices of the backbone length Lb, to exclude that the data are strongly affected by finite size artifacts. The straight line indicates that the data are compatible with a simple linear relation, ξ−1(N, 0) ∝ 1/N .

an unmixed binary (A,B) homopolymer blend: for this problem it is well-known (see Werner et al. [109] for ref- erences) that the shape of the diblocks is dumbbell like, the A-block being stretched away from the interface, in order to be embedded in the A-rich phase underneath of the interface, and the B-rich block also being stretched away from the interface, in order to be embedded in the B-rich phase above the interface. As a consequence of our discussion, we call into

question the idea of the “Janus cylinder”-type phase separation [56, 57, 58] and propose as an alternative pos- sibility (Figure 32) the “double cylinder” (with cross sec- tion resembling the number 8). Which of these cross- sectional structures occur will depend on the interac- tion parameters AA = BB, and AB, of course. If the strength of the attractive interactions |AA| = |BB| exceeds the strength of the repulsion |AB| sufficiently much, it is clear that for T → 0 the Janus cylinder type phase separation will occur, while in the opposite limit, when |AB| exceeds |AA| = |BB| sufficiently much, the double cylinder geometry will win. In the macroscopic continuum limit a comparison of the respective surface energies would imply that the double cylinder geometry, which avoids an AB interface, but requires for the same volume taken by